# Engineering Manual (8½" x11")

```SYMBOLS AND UNITS
THORDON ELASTOMERIC BEARINGS
ENGINEERING MANUAL VERSION E2006.1
SYMBOLS AND UNITS
Units
Metric
Imperial
APPROXIMATE COMPARISON OF
VARIOUS HARDNESS SCALES
Ct
= Thermal Expansion
Allowance
mm
inches
Cs = Absorption Allowance
mm
inches
d
= Shaft diameter
mm
inches
Eo = Modulus of elasticity
MPa
psi
I.D. = Inside diameter of bearing
mm
inches
O.D. = Outside diameter of bearing
mm
inches
L
= Length of bearing
mm
inches
N
= Shaft speed
R.P.M.
R.P.M.
P
= Pressure
MPa
psi
Ta = Machine Shop Ambient
Temperature (Nominally
21&deg;C (70&deg;F))
&deg;C
&deg;F
To = Operating temperature
&deg;C
&deg;F
W.T. = Wall thickness of bearing
mm
inches
α
= Coefficient of thermal
expansion
cm/cm/&deg;C in./in./&deg;F
&micro;
= Coefficient of friction
V
= Velocity
m/sec.
ft./min.
γ
= Poisson’s Ratio
FREEZE FIT COOLANT TEMPERATURES
Dry Ice: -78&deg;C (-109&deg;F)
Liquid Nitrogen: -196&deg;C (-320&deg;F)
Note: All clearances referred to in this manual are diametrical clearances
METRIC CONVERSION TABLE
• Length
1 Metre (m) = 39.37 Inches (in.)
1 Millimetre (mm) = 0.03937 Inches (in.)
• Force
1 Newton (N) = 0.2248 lbs.
1 Kilogram (kg) = 2.205 lbs.
• Pressure
* 1 kg/cm2 = 14.223 psi (lbs./in.2)
** 1 Mega Pascal (MPa) = 145 psi (lbs./in.2)
1 N/mm2 = 145 psi (lbs./in.2) = 1 MPa
1 MPa = 10.195 kgf/cm2
1 Bar = .981 kg/cm2
1 Mega Pascal (MPa) = 10 Bar
* Kilo = 1,000
** Mega = 1,000,000
OTHER THORDON
TECHNICAL INFORMATION AVAILABLE
a) Thordon Bearing Installation Manual
b) Thordon Water Lubricated Propeller Shaft Bearing
Design Manual
c) Thordon Bearing Sizing Calculation Program
d) ThorPlas&reg; High Pressure Bearing Engineering Manual
Thordon Bearings Inc. if you require any of the above.
WARRANTY
LIMITED WARRANTY AND LIMITATION OF LIABILITY
FOR THORDON BEARINGS INC. (‘TBI’)
(a) Basic Terms. TBI provides a limited warranty on the
Goods of its own manufacture sold by it to the Buyer
thereof, against defects of material and workmanship
(the “Limited Warranty”).
(b) Coverage. This Limited Warranty covers the repair
or replacement or the refund of the purchase price,
as TBI may elect, of any defective products regarding
which, upon discovery of the defect, the Buyer has given
immediate written notice. TBI does NOT warrant the
merchantability of its product and does NOT make any
warranty express or implied other than the warranty
contained herein.
(c) Third Party Products. Accessories, equipment and
parts not manufactured by TBI are warranted or otherwise guaranteed only to the extent and in the manner
warranted or guaranteed to TBI by the actual
manufacturer, and then only to the extent TBI is able
to enforce such warranty or guarantee.
(d) Limited Liability. TBI’s liability for any and all claims,
damages, losses and injuries arising out of or relating to
its performance or breach of any contract of sale of goods
and the manufacture, sale delivery, re-sale, repair, or use
of any goods, shall NOT exceed the agreed price of such
Goods. The Buyer’s remedy shall be at TBI’s option, the
replacement or repair of the Goods. This shall be the
Buyer’s sole, exclusive and only remedy against TBI. IN NO
EVENT SHALL TBI BE LIABLE FOR INCIDENTAL, SPECIAL OR
CONSEQUENTIAL DAMAGES, INCLUDING BUT NOT LIMITED
TO LOSS OF PROFITS, BUSINESS, GOODWILL, INCURRING
OF MACHINERY DOWNTIME, DESTRUCTION OR LOSS OF ANY
CAPITAL GOODS, LIABILITY FOR PERSONAL INJURY, DEATH,
PROPERTY DAMAGE AND ANY OTHER TYPE OF DAMAGES
WHETHER SIMILAR TO OR DIFFERENT FROM THIS LISTING.
(e) Latent Defects. In cases of defects in materials or
workmanship or defects arising from the selection of
material or processes of manufacturer, such defects must
be apparent in the Goods within three (3) months, after
delivery and acceptance of the Goods to the Buyer.
(f) Exclusions. TBI shall, as to each aforesaid defect, be
relieved of all obligations and liability under this Limited
Warranty if:
2. The Goods shall not be operated or maintained in
accordance with TBI’s written instructions as delivered
to the Buyer, at any time or from time to time,
unless the Buyer furnishes reasonable evidence
that such operation or maintenance was not a cause
of the defect;
3. The Goods shall not be operated or maintained
under normal industry use, unless the Buyer furnishes
reasonable evidence that such operation was not a
cause of the defect;
4. The Goods shall have been repaired, altered or
modified without TBI’s written approval or, if the
Goods shall have been operated subsequent to its
involvement in an accident or breakdown, unless the
Buyer furnishes reasonable evidence that such repair,
alteration, modification, operation, accident or
breakdown was not a cause of the defect; provided,
however, that this limitation insofar as it relates
to repairs, accidents and breakdowns, shall NOT be
applicable to routine repairs or replacements or minor
accidents or minor breakdowns which normally occur
in the operation of a machine, if such repairs or
replacements are made with suitable materials and
according to standard practice and engineering;
5. The Buyer does not submit reasonable proof to TBI
that the defect is due to a material embraced within
TBI’s Limited Warranty hereunder.
(g) Warranty Term. This Limited Warranty made by TBI
contained in these Terms and Conditions, or contained in
any document given in order to carry out the transactions
contemplated hereby, shall continue in full force and
effect for the benefit of the Buyer, save and except, no
the date which is twelve (12) months following delivery
and acceptance of the Goods pursuant to this Contract.
(h) Expiration and Release. After the expiration of this
Limited Warranty’s period of time, as aforesaid, TBI shall
be released from all obligations and liabilities in respect
of such warranty made by TBI and contained in this
Contract or in any document given in order to carry out
the transactions contemplated hereby.
1. The Goods are operated with any accessory,
equipment or part not specifically approved by TBI
and not manufactured by TBI or to TBI’s design and
specifications, unless the Buyer furnishes reasonable
evidence that such installation was not a cause of
the defect; provided, that this provision shall not
apply to any accessory, equipment or part, the use
of which does not effect the safety of the Goods;
53
INDEX
INDEX
1. THORDON DEFINITION . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2
2. TRIBOLOGY
a) Friction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3
b) Lubrication . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3
c) Wear . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5
3. PHYSICAL PROPERTIES
a)
b)
c)
d)
e)
f)
g)
h)
i)
j)
k)
Thermal Effects . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Effect of Water or Oil . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Shape Factor . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Stress Strain . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Stiffness . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Compression Set - Creep - Stress Relaxation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Shear . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Impact/Resilience . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Hysteresis . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Chemical Resistance . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Typical Physical Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
7
8
8
9
9
10
10
10
11
11
12
4. DESIGN GUIDE
a) Application Analysis . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
b) Bearing Pressure . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
c) Velocity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
d) PVT Graphs . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
e) Length/Diameter (L/D) Ratio . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
f) Wall Thickness . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
g) Lubrication Grooves . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
h) Mating Surface . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
i) Fitting . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
j) Machining Tolerances . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
k) Minimizing Initial Installed Clearance . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
l) Selection Process . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
m) Problems &amp; Causes of Bearing Failure . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
13
13
13
13
18
18
19
19
20
22
22
23
25
5. APPLICATION DESIGN FOR THORDON BEARINGS
a)
b)
c)
d)
e)
f)
g)
h)
i)
j)
k)
l)
m)
n)
Application Design . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Interference . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Bonding . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Bore Closure . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Running Clearance . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Thermal Expansion Allowance . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Absorption Allowance . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Minimum Installed Clearance . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Using the Thordon Bearing Sizing Calculation Program . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Step by Step Manual Calculations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Sample Manual Calculations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Keyed Tubular Bearing Calculations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
High Pressure Bearings . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Vertical Pump Bearings: Dry Start-up . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
27
27
30
30
31
33
33
34
34
36
37
38
39
40
6. MACHINING &amp; MEASURING
a)
b)
c)
d)
General Machining . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Machining XL, SXL or COMPAC . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Machining Composite . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Dimensional and Surface Finish Measurements . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
41
41
46
47
APPENDIX 1
Bonding with TG-75 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 49
1
THORDON DEFINITION
1) THORDON DEFINITION
Thordon elastomeric bearing material is made from
thermosetting resins which are three dimensional, crosslinked condensation polymers. Thordon is a very hard,
tough synthetic polymer alloy that has performance
characteristics superior to those of most other bearing
materials, both metallic and non-metallic. Thordon
performs particularly well, compared to other materials,
in applications where it is exposed to, or submerged in,
water, in extremely dirty environmental conditions, and
are two basic reasons for this superior performance. First,
Thordon, an elastomer, returns to its original shape after
being compressed or deformed under normal operating
conditions. Second, due to the basic characteristics of
the material, Thordon has a high natural resistance to
abrasion. These two characteristics result in exceptional
performance and long life in a number of difficult and
dirty environmental conditions in both marine and
industrial applications.
Thordon Bearings produces several bearing grades that
offer specific operating advantages in different
applications. The grade and colour are noted as follows:
XL (black)
SXL (off-white)
COMPAC (orange)
Composite (yellow outer shell, black bearing wear
surface [known as GM2401])
HPSXL (grey)
HPSXL TRAXL (HPSXL bonded in a metallic shell)
ThorPlas&reg; (blue) - covered in separate manual
Thordon, developed and manufactured by Thordon
Bearings Inc. in Burlington, Ontario, Canada, was
introduced to the Canadian market in 1966. It is now
sold through factory trained stocking distributors and
agents in over 70 countries worldwide.
2
This Engineering Manual has been prepared based on
the company’s many years of experience in manufacturing
and installing Thordon bearing products worldwide.
This information is offered as part of our service to
customers. It is intended for use by persons having
technical training and skill, at their discretion and risk.
The company reserves the right to change or amend any
specification without notice. The sole, exclusive and only
responsibility of Thordon Bearings Inc. (’the Company’)
to any customer or distributor of the Company’s products
for any claims, damages, losses or liabilities arising out
of, or relating to, any products supplied by the Company,
and the Company’s sole, exclusive and only warranty shall
be in accordance with the Company’s Limited Warranty
and statements limiting its liability set out on page 53
of this manual. In no event whatsoever shall the Company
be liable for special, indirect or consequential damages.
TRIBOLOGY
2) TRIBOLOGY
Thus, if the load on the shaft is increased, then the
friction force will increase, along with the frictionally
generated heat. If the heat cannot be dissipated to
a large heat sink or through a lubricant, the surface
temperature of the bearing will rise. Because Thordon,
like many other synthetic bearing materials, is a poor
conductor of heat, the dissipation of frictional heat
is a significant consideration in bearing design.
a) Friction
b) Lubrication
c) Wear
Tribology is the scientific study of friction, lubrication
and wear. It comes from the Greek word ‘Tribos’ which
means ‘to rub’.
b) LUBRICATION
a) FRICTION
i)
Wet Lubrication
Friction is usually defined as a force that resists the
motion of an object. With a Thordon bearing, friction
occurs when a shaft applies a load to a bearing. When
the shaft turns, the friction between the shaft and bearing
resists the rotation and therefore a certain amount of
torque is required to keep it turning. This torque does
not do any useful work and is converted into heat.
The magnitude of the friction force F (f) is dependent
on a value called the coefficient of friction (&micro;) and the
‘normal’ applied load (N). The relation is as follows:
F (f) = &micro; (N)
Friction is almost always undesirable (except for
applications like brakes, clutches and tires). It often leads
to problems with overheating, high wear and high running
cost. In order to reduce friction, lubrication is employed.
Lubrication is the act of applying a substance, usually
a liquid, between two moving surfaces, with the primary
aim of reducing friction and/or wear and the secondary
aim of carrying away heat. When a bearing is ‘wet’
lubricated, friction becomes highly dependent on speed
and lubricant properties as demonstrated by the two
examples in Figure 1.
Figure 1: Typical Oil / Water Cross-Over Friction Curve
.25
Typical white metal bearing/oil
Thordon COMPAC bearing/ water
COEFFICIENT OF FRICTION
.2
.15
.1
.05
0
0.25
50
0.50
100
1.00
200
1.50
300
2.00
400
2.50
500
3.00
600
3.50
700
4.00
800
4.50 (m/sec)
900 (ft/min)
SHAFT VELOCITY
3
TRIBOLOGY
Figure 1 demonstrates the results of testing with a
Thordon water lubricated COMPAC bearing and also
a typical oil lubricated white metal bearing. The oil
lubricated bearing starts with a lower friction level,
which then drops very rapidly to its lowest friction
level before slowly climbing back up.
The friction force for water lubrication starts higher
because of water’s poor lubricity and requires a higher
speed to achieve hydrodynamic operation. This is due
to the low viscosity of water.
An interesting observation is that in the high-speed
range, the water lubricated frictional force is actually
lower than with oil. Once hydrodynamic operation is
achieved, friction increases. However, the higher viscosity
of oil results in greater shearing forces and higher friction
than with water.
This is illustrated by a typical “Stribeck curve” (Figure 2)
which plots the coefficient of friction against the
hydrodynamic parameter Zn/P. The curve is divided into
three main lubrication regimes.
Figure 2. The Stribeck curve, illustrating
the buildup of hydrodynamic film
Mixed
Regime
Full Film
(Hydrodynamic)
Regime
Coefficient of Friction
Boundary
Regime
(Viscosity X Speed) / Load or Zn/P
In the first (Boundary) regime, direct contact exists
between the shaft and the bearing resulting in high
friction values. In this region of the curve, high bearing
self-lubricity is of significant benefit. As the shaft speed
increases we move into the second (Mixed film) regime
of the curve where the hydrodynamic film starts to build
and effectively “lift” the shaft from the bearing surface.
The result is less shaft to bearing contact and friction
drops rapidly. Further increases in speed take us into
the third (Hydrodynamic) regime where the hydrodynamic
film builds sufficiently to eliminate all direct contact.
As speed continues to increase, friction begins to increase
because of the increasing shear resistance imparted by
the viscosity of the lubricant.
4
The transition between lubrication regimes during
operation of a bearing depends primarily on lubricant
properties, velocity and load. The curve profile and
definition of transition points will depend on the bearing
geometry, clearance ratio, self-lubricity of the bearing
material and surface finish. A higher viscosity lubricant
results in the generation of a hydrodynamic film at a
lower shaft speed and effectively moves the transition
points to the left. Increasing the viscosity, however, also
increases the minimum operating coefficient of friction.
Lowering the coefficient of friction of the bearing material
results in decreased friction at shaft speeds below the
point where full hydrodynamic operation occurs. The
geometry of the bearing, and in particular, whether the
bearing is grooved also affects the curve. A continuous
bearing surface without grooves allows the hydrodynamic
film to build quicker than one with grooves. Hydrodynamic
calculations show that the necessary speed to achieve
a hydrodynamic film is double that for an ungrooved
bearing.
Wet lubrication also has the added benefit of being able
to carry away frictionally generated heat, the enemy of
all bearings. This is especially significant with Thordon
because the low thermal conductivity of the material
does not allow much heat to be dissipated through the
bearing wall (metallic bearings have much higher thermal
conductivity and can dissipate more heat through the
bearing wall). Wet lubrication can be supplied by several
methods varying in complexity and performance. There
are drip feed systems (normally oil), which are appropriate
for slow to intermediate speeds where heat build up is not
a concern. Bath systems are also used - where the bearing
is fully or partially submerged in a limited quantity of
lubricant. The limiting factor with bath systems is that
the whole bath can become overheated if the assembly
generates significant heat. A third method is a continuous
flow of fresh cool lubricant from an external source,
usually force-fed. This method is essential for applications
such as marine propeller shafts, vertical pumps and
to levels of heat generation which cannot be dissipated
by a bath of lubricant.
NOTE: WATER FLOW REQUIREMENTS
A Thordon bearing application involving full rotation
may require water flow for lubrication and cooling.
If required, the minimum recommended flow rate is
0.15 litres per minute per millimetre (1 U.S. gal. per
minute per inch) of shaft diameter. The water should
be as clean and cool as possible. “Cooling” water
above 40&deg;C (104&deg;F) should be avoided.
TRIBOLOGY
ii) Grease
ii) Abrasive Wear
Grease is a form of lubrication that lowers friction
and allows a lubricant film to form. Grease does not
have the ability to carry away heat. Fresh grease is
applied on a periodic basis to lubricate the bearing
and purge the old grease and debris. Periodic lubrication
is required to avoid dry running conditions. Grease
lubrication of Thordon bearings should be limited to
relatively clean environments where heat generation
is not a significant problem (see PVT Graph: Figure 13f).
Abrasive wear involves the wearing of a softer surface
by a hard particle. Examples are sandpaper or a grinding
wheel (two body abrasion) or sand particles between
a bearing and a shaft (three-body abrasion). Actual
abrasive wear will vary with the quantity of abrasives
present and with the size, shape and composition of
the abrasive particles.
iii) Non-Lubricated – Dry Running
Thordon can be specified as non-lubricated for relatively
low speed applications where regular lubrication is not
possible or where abrasives may be attracted to grease
lubrication. Thordon SXL exhibits the best properties
for dry running due to the high lubricant content of its
formulation. This reduces friction and heat generation.
Where the pressure on the bearing is beyond the
acceptable limit for Thordon SXL, Thordon HPSXL can
be considered. It can run dry but does not have as good
abrasion resistance as SXL. For even higher pressure
dry running applications, a thin wall of HPSXL bonded
in a metallic shell or ThorPlas&reg; are available.
iv) Pressure Velocity Time (PVT) Curves
Selection of the appropriate method of lubrication
can be facilitated by referring to the various PVT
(pressure, velocity, time) curves in the Design Guide
Section of this manual.
c) WEAR
Wear is the destructive removal of material from
contacting surfaces moving relative to one another.
Wear can take several forms and, as a highly complex
process, is difficult to predict.
i)
Adhesive wear occurs when minute peaks of two rough
surfaces contact each other and weld or stick together,
removing a wear particle. Adhesive wear of Thordon
is very minimal at normal temperatures and pressures,
but becomes the dominant wear mode as the operating
temperature reaches maximum operating limits. The
maximum operating temperatures for Thordon are defined
to try and avoid this mode of wear. The amount of
adhesive wear is related to the friction between the two
surfaces, the pressure on the working surface, and the
type and amount of lubrication provided.
Typical example of bearing with abrasive wear.
The best approach to minimizing abrasive wear is to
reduce or eliminate the quantity of abrasives by using
filters or clean water injection. If this is not possible,
then a satisfactory alternative for minimizing abrasive
wear is to have one surface very hard and the second
relatively soft and compliant. Abrasive particles are
allowed to be pushed into the softer surface and roll
or slide through the contact area with very little damage
to the shaft or bearing. The elastomeric nature of Thordon
bearings facilitates abrasive wear resistance because
the material flexes when it encounters abrasive particles.
With shaft rotation the particles are moved along the
bearing surface until flushed out through a lubrication
groove. With more rigid materials the abrasive particles
tend to become embedded in the material and may cause
shaft wear.
A continuous flow of fresh lubricant (as in a propeller
shaft application), and grooves in the Thordon bearing,
will help to flush out abrasive particles and reduce
the amount of abrasive wear. Tests have shown that
optimum life in an abrasive environment for a water
lubricated bearing was obtained with a very hard shaft,
a Thordon Composite bearing and a continuous flow of
lubricating water.
5
TRIBOLOGY
iii) Wear Comparison
An independent test lab at the University of Cincinnati
(USA) has done extensive wear testing of Thordon and
other bearing materials. All the bearing materials were
compared in tests on a specially designed machine
using a circulating abrasive slurry – see Note, Figure 3.
The comparative results are illustrated in Figure 3.
Figure 3: Typical Bearing Abrasive Wear Rates
Projected Bearing Wear Volume (cc/24 hours)
NOTE: Wet third particle abrasion.
Shaft Material: carbon steel
Bearing I.D.: 2.5 cm (1 in.)
Abrasive slurry mixture: 2% bentonite, 6% sand, 6% clay, 86% water
6
PHYSICAL PROPERTIES
a) Thermal Effects
b) Effect of Water or Oil
c) Shape Factor
d) Stress Strain
e) Stiffness
f) Compression Set - Creep Stress Relaxation
g) Shear
h) Impact Resilience
i) Hysteresis
j) Chemical Resistance
k) Typical Physical Properties
a) THERMAL EFFECTS
ii) Coefficient of Expansion/Contraction
The coefficient of thermal expansion/contraction for
Thordon is non-linear, like other non-metallics, and
varies throughout its temperature range. Figures 4 &amp; 5
show typical results of Thordon materials which exhibit
lower coefficients of contraction than of expansion.
The coefficient of thermal expansion for HPSXL is
12 x 10-5 &deg;C (6.7 x 10-5 &deg;F)and does not exhibit the
same non-linearity of SXL, COMPAC and XL.
Figure 4: Dimensional Change (%)
Vs. Temperature – THORDON XL and GM2401
2.5%
2.0%
% DIMENSIONAL CHANGE
3) PHYSICAL PROPERTIES
1.5%
1.0%
0.5%
0%
i)
Temperature Limits
–0.5%
–100 DRY ICE –50
(–148) –78˚C (–58)
(–109)
All bearings are subjected to the combined effects of the
ambient environmental temperature and the frictional
heat generated during operation. Thordon, like all other
non-metallic materials, has a low thermal conductivity
compared to metal so allowances must be made to limit
frictional heat build up.
The lower operational limit of Thordon is -60&deg;C (-80&deg;F).
It is possible, however, during shrink fitting to use liquid
nitrogen at a temperature of -195&deg;C (-320&deg;F) without
Thordon becoming too brittle to fit.
The upper temperature limit for Thordon operating in
a wet environment is 60&deg;C (140&deg;F) due to Hydrolysis.
Hydrolysis is explained in more detail in the following
subsection b) Effect of Water or Oil. This limit also applies
to other liquids with a significant aqueous content.
For bearings lubricated with standard mineral grade oil,
the upper temperature limit is 75&deg;C (170&deg;F).
50
(122)
100
(212)
TEMPERATURE ˚C (˚F)
COEFFICIENT OF EXPANSION FOR TEMPERATURE RANGE
&lt;0˚C (32&deg;F):
0˚C to 30˚C:
(32˚F to 86˚F)
10.2 x 10 -5 (˚C)
5.7 x 10 -5 (˚F)
14.8 x 10 -5 (˚C)
8.2 x 10 -5 (˚F)
&gt; 30˚C (86&deg;F):
18.1 x 10 -5 (˚C)
10.1 x 10 -5 (˚F)
Figure 5: Dimensional Change (%)
Vs. Temperature – THORDON SXL and COMPAC
3.0%
% DIMENSIONAL CHANGE
The upper temperature limit for Thordon operating in a
non-aqueous environment is 105&deg;C (225&deg;F). Above 105&deg;C
(225&deg;F), softening of the surface occurs. As the surface
softens, the coefficient of friction increases. This in
turn results in additional heat being generated. The
temperature increases further and the process continues
until the bearing fails. In some cases this may be arrested,
as may occur with misalignment, provided a quenching
medium is supplied.
0
(32)
2.0%
1.0%
0%
–1.0%
–100 DRY ICE –50
(–148) –78˚C (–58)
(–109)
0
(32)
50
(122)
100
(212)
TEMPERATURE ˚C (˚F)
COEFFICIENT OF EXPANSION FOR TEMPERATURE RANGE
&lt;0˚C (32&deg;F):
0˚C to 30˚C:
(32˚F to 86˚F)
10.9 x 10 -5 (˚C)
6.1 x 10 -5 (˚F)
15.1 x 10 -5 (˚C)
8.4 x 10 -5 (˚F)
&gt; 30˚C (86&deg;F):
21.1 x 10 -5 (˚C)
11.7 x 10 -5 (˚F)
7
PHYSICAL PROPERTIES
b) EFFECT OF WATER OR OIL
i) Water Absorption
Thordon expands in water approximately 1.3% by volume
under atmospheric conditions at a temperature of 21&deg;C
(70&deg;F) due to the isotropic nature of the polymeric
structure. At this temperature or less, full expansion
may take 6 to 18 months depending upon geometry.
Should the temperature be increased, not only does
the volumetric absorption percentage increase, but
also the rate of absorption. In tests using water at
60&deg;C (140&deg;F) the volumetric absorption increased
to 2.0% within 100 hours.
In order to determine the effects of water absorption
on Thordon as it relates to a bearing press fitted in
a housing, a series of tests were performed. These
tests showed the approximate average effects of water
absorption on both bore closure and axial length at
21&deg;C (70&deg;F). The average effect on bore closure is .011
multiplied by the wall thickness. The average effect on
axial swell is .005 multiplied by the length of the bearing.
ii) Hydrolysis
When Thordon is subjected to continuous immersion
in hot water, i.e. above 60&deg;C (140&deg;F), the material
chemically deteriorates over time due to a reaction with
the hot water. This deterioration or breakdown is known
as hydrolysis. The surface of the material softens initially
and then eventually cracks and breaks. Hydrolysis will
also occur with other liquids with a high aqueous content.
volumetrical absorption needs to be considered. For
example, at 75&deg;C (167&deg;F), the volumetrical expansion
can be above 2.5%.
In practice, the dimensional allowances used for water
lubricated bearings are also used for oil lubricated
bearings. This is partially because of concern for the
lower thermal conductivity of oil compared to water.
When a different type of lubricating oil is used, it
should be tested for compatibility with Thordon before
installation of the bearing. Thordon may react differently
to non-standard lubricating oils. A significant change
in dimensions (beyond that expected for water), or
softening after immersion in the lubricant for more
than 24 hours will indicate that the lubricant is not
compatible with Thordon.
c) SHAPE FACTOR
Compression testing of elastomers has determined that
the stress strain curve is greatly affected by the shape of
the part. This effect is known as the Shape Factor and is
determined by dividing the loaded area by the area free to
bulge. For a given load, as the shape factor increases the
resulting deflection of the elastomer decreases. The load
bearing capacity of an elastomer is limited by the amount
of deflection it can accept, so increasing the shape factor
enables the elastomer to support more load.
Figure 6
BEARING
PROJECTED
AREA
WALL
THICKNESS (1)
Typical example of bearing with hydrolysis.
iii) Absorption of Oil
Absorption by Thordon elastomers of standard mineral
grade lubricating oil is slow and to a small extent,
particularly at low temperatures such as 22&deg;C (72&deg;F).
Dimensional changes are small and their consideration
is less important than those in water at such temperatures. However, in high operating temperatures,
8
I.D
.
H
LENGT
How the shape factor relates to a sleeve bearing is
important. Figure 6 indicates how the calculation
is applied to a bearing retained in a housing.
∴ Shape Factor = Length of Bearing
2 x Wall Thickness
Using the shape factor equation, it can be seen that if
the thickness is reduced, the shape factor will increase.
The shape factor used in most Thordon testing is 8. The
results and method of testing are shown in the following
sub section, d) Stress Strain.
PHYSICAL PROPERTIES
d) STRESS STRAIN
When a load is applied to Thordon elastomeric bearings,
they move in accordance with the force exerted. In
compression, the volume will not significantly change,
but there can be a significant change to the shape.
The normal stress strain curves are determined
experimentally using a tensile test machine and a standard
test sample. However, in order to develop data more
decided to test the material in the compressive mode
using a full bearing form.
Figure 7
2&quot; dia.
STEEL
SHAFT
HYDRAULIC RAM
HOUSING
DIAL INDICATOR
BEARING
In compression, the Stress-Strain Curve for Thordon in
Figure 8 is dependent on the shape factor of the material
and it’s ability to move against the mating material.
For the same deflection, a bonded sample will carry more
load than a sample where the bearing can expand axially.
If lubrication is added to the mating surface allowing
the curve is expected to be flatter than if the mating
surface is dry.
Using a shape factor of 8, testing indicated a maximum
deflection limit of 1.25% for full rotation installations,
and 4% for oscillating motion. Beyond these limits,
bearing performance may deteriorate. These limits do not
take into consideration any frictional heat generated by
shaft movement.
By taking the shape factor concept to its logical
conclusion, it is possible to design Thordon sleeve
bearings capable of operating at high pressures. The
Thordon HPSXL TRAXL bearing, for example, develops very
high shape factors by bonding a thin layer of Thordon
HPSXL into a metallic shell. Depending on the operating
as high as 70 MPa (10,000 psi).
Thordon XL, SXL and COMPAC are true elastomers and
as such do not have an ultimate compressive strength.
DIAL INDICATOR
&quot;V&quot; BLOCKS
e) STIFFNESS
Figure 7 shows how the bearing was loaded and how the
deflection was measured. Note that the shaft deflection
was subtracted from the housing deflection in order to
obtain net bearing deflections.
Stress-StrainCURVES
Curves
Figure 8: Thordon
THORDON
STRESS-STRAIN
6000
Bearing stiffness is dependent on both size parameters
and physical properties. The size parameters are the
bearing length, diameter and wall thickness. The physical
property to be considered is the Young’s Compressive
Modulus (Eo) of the bearing material, which is equal
to compressive stress divided by compressive strain.
Stiffness
42.0
4000
35.0
28.0
XL
ON
D
OR
TH
3000
N
DO
L
SX
21.0
OR
TH
2000
14.0
1000
7.0
0
1
2
3
4
5
BEARING PRESSURE (MPa)
maximum deflection
for full rotation
5000
BEARING PRESSURE (psi)
maximum deflection
for limited rotation
where:
6
DEFLECTION (percentage of wall thickness)
BORE: 2.0&quot;
50mm
LENGTH: 2.5&quot;
WALL THICKNESS: 0.155&quot;
65mm
4.0mm
SHAPE FACTOR: 8.0
= (L x D x Eo)/t
L = Bearing Length: mm (in.)
D = Bearing Diameter: mm (in.)
Eo = Young’s Compressive Modulus: MPa (psi)
t = Wall Thickness (W.T.): mm (in.)
Figure 9: Compressive Modulus of Elasticity (Eo )
Material
Eo (MPa)
Eo (psi)
Rubber*
Thordon SXL
Thordon COMPAC
Thordon XL
Thordon HPSXL
Laminated Phenolic
White Metal
Steel
103
440
440
490
650
1,730
33,500
206,900
15,000
64,000
64,000
71,000
94,250
251,000
4,860,000
30,000,000
*of a hardness typically used in bearings
8.0
FIG. 9
9
PHYSICAL PROPERTIES
For bearings with equal size parameters the bearing
stiffness is directly proportional to the value of Young’s
Compressive Modulus for the material. The previous
chart gives the value of Eo, Young’s Compressive Modulus,
for various materials commonly used as bearings.
Based on Figure 9, a Thordon XL bearing would be 4.7
times stiffer than rubber, assuming that the bearings
are of equal sizes and shape factor.
NOTE: The bearing shape factor was assumed to be 8 for these
calculations. For elastomeric materials, the effective Compressive
Modulus of Elasticity, Eo, increases a small amount for correspondingly
large increases in shape factor. Therefore, the values of stiffness
assumed are estimated to be accurate to +/- 20% over a wide range
of bearing shape factors.
In engineering calculations, the stiffness of bearing
support structures is typically in a range between 0.5
to 1.0 MN/mm (2.8 to 5.7 x 106 lbs./in.). This is much
less than the typical bearing material stiffness of 5.0
to 20.0 MN/mm (28.0 to 112.0 x 106 lbs./in.). The
typical stiffness of Thordon is approximately 5 MN/mm
(28 x 106 lbs./in.) and the typical water film stiffness is
approximately 50 MN/mm (280 x 106 lbs./in.). As a result,
the stiffness of the bearing material is normally not
considered in shaft whirling vibration calculations.
When rubber bearings are being specified, due to the low
stiffness characteristics of rubber (20% to 25% of that
of Thordon), shaftline designers may be accustomed to
considering the bearing flexibility when making whirling
vibration calculations. However, this is not the case with
Thordon XL, SXL, COMPAC or HPSXL where, due to a much
higher stiffness, the Thordon bearing can be assumed to
be as stiff as the bearing support structure.
f) COMPRESSION SET - CREEP STRESS RELAXATION
i)
Compression Set
Compression set or permanent set is the residual
deformation remaining after the removal of the deforming
compressive stress. Under normal Thordon bearing
operating conditions, compression set is not a problem.
Please consult with Thordon Bearings if a Thordon bearing
will be exposed to constant high pressure combined with
temperatures above 50&deg;C (122&deg;F).
To reduce compression set, the shape factor should be
increased. This reduces the initial deflection and therefore
the amount of possible compression set. Increasing the
shape factor is especially important when the pressure
is in excess of 10 MPa (1450 psi). In such applications,
Thordon HPSXL TRAXL or ThorPlas&reg; bearings should be used.
10
ii) Creep
When an elastomer is subjected to a load, it will deform
proportionally to that load and in inverse proportion to
the shape factor. Some deformation will also continue
with time. This effect is known as ‘creep’. In the normal
operating range of Thordon bearings, creep is not a
significant factor. As with compression set, it only
becomes significant when bearings are continuously
exposed to high pressure and high temperature. The
amount of creep, like compression set, can be reduced by
increasing the shape factor as the load increases, thereby
reducing strain for any given pressure.
iii) Stress Relaxation
Stress relaxation is the direct result of creep and varies
depending on the stress level. Stress relaxation is usually
expressed in terms of percentage stress remaining after
a specified period of time at a given temperature.
This factor is significant when calculating dimensions
for interference fit bearings. The interference must be
sufficient to ensure that adequate retention force exists
over time.
It has been determined by testing that Thordon bearings
can lose their interference fit (by stress relieving) in the
housing when subjected to elevated temperatures. Thordon
SXL and COMPAC stress relieve at temperatures greater
than 60&deg;C (140&deg;F) while Thordon XL and Composite stress
relieve at temperatures greater than 80&deg;C (175&deg;F).
Bearings exposed to temperatures above these levels
should not be fitted using an interference fit. Bonding
is the recommended alternative.
g) SHEAR
The shear force on a sleeve bearing is a function of the
coefficient of friction between the bearing, the shaft
and the nominal load. When bearings are installed using
an interference fit, the relative force is sufficient to
prevent rotation. If the friction force or normal load
should increase dramatically, such as an accumulation
of significant abrasives, the shear force may exceed
the retention force. If there are concerns regarding
Thordon Bearings.
h) IMPACT/RESILIENCE
Thordon, which possesses high impact strength, has the
ability to absorb shock loads and the resilience to return
to its original shape. Resilience is defined as the ratio
of energy given up in recovery from deformation to the
energy required to produce the deformation. This
combination allows Thordon to resist pounding out of
shape which frequently occurs and can lead to failure with
PHYSICAL PROPERTIES
white metals or plastics. At almost 10 times the impact
strength of nylon, Thordon is virtually unbreakable!
In applications where there are significant low frequency
impact loads, the bearing should be designed with a
heavier wall thickness.
i) HYSTERESIS
Hysteresis is a type of dynamic failure due to high
frequency flexing. The failure occurs when the material
absorbs an impact load and, before the material can fully
recover from the first impact, it is subjected to a second
one. The result is an energy build up below the surface
of the material in the form of heat. This heat, if allowed
to accumulate, will eventually damage the material.
Hysteresis is the percentage energy loss per cycle of
deformation and can be measured as the difference
between the percentage resilience and 100%.
Thordon, due to the nature of its formulation, can be
subject to damage by hysteresis. If the application
being considered will subject Thordon to dynamic impact
considerations that will minimize the potential for
problems. Figure 10 illustrates that increasing the shape
factor (reducing the wall thickness) will reduce the
deflection and increase the rate of recovery thus reducing
heat creation and build up. A thinner wall thickness also
allows increased dissipation of heat through the bearing
wall to the housing to reduce the amount of heat build up.
INCREASING TEMPERATURE
Figure 10: Effects Of Hysteresis
CO R
E TE
MP
ERA
TU
RE
SURFACE
TEMPE
RATU
RE
DECREASING WALL THICKNESS
(INCREASING SHAPE FACTOR)
j) CHEMICAL RESISTANCE
Thordon is non-corrosive and is resistant to oil, water and
most chemicals. It is not affected by lubricants normally
used with sleeve bearings.
Thordon is unaffected by mild acid or caustic baths
(pH range of 2-7) or other chemical environments which
would be harmful to metallic bearings. See the general
Chemical resistance guide in Figure 11.
For critical applications it is recommended that an
immersion test be performed to determine whether or
not Thordon will be safe to use. Significant softening
or dimensional changes after twenty-four hours of
immersion at application temperatures will indicate
that Thordon is unsuitable for that application.
distributor or Thordon Bearings Inc.
Figure 11:
Thordon Chemical Resistance Chart
Chemical/Fluid
Thordon
Salt solutions
Sodium chloride
Weak acids
Acetic acid
Lactic acid
Strong acids
Sulphuric, 5%
Sulphuric, concentrated
Hydrochloric, 10%
Weak bases
Ammonia 10% Aq.
Sodium carbonate
Triethanolamine
Strong bases
Sodium hydroxide, 10%
Oxidizing agents
Hydrogen peroxide, 1-3%
Chromic acid
Hydrocarbon/fuels
Aromatic – benzene, toluene
Aliphatic – gasoline, grease
Lubricating oils (petroleum)
Chlorinated solvents
Alcohols
Ethanol
Methanol
Ketones
Methyl ether ketone
Acetone
Ethers
Diethyl ether
Esters
Ethyl acetate
Methyl acetate
Freon 12
Vegetable Oils
A: Excellent-No Affect;
C: Fair-Moderate Affect;
A
A
B-D
D
B
B-D
B-C
D
B
A-B
A
B
B-D
B
B
B-C
B
C
A-B
B
A-B
B
D
D
D
D
D
D
D
D
D
D
D
D
A-C
A-B
B: Good-Little Affect;
D: Unacceptable
11
PHYSICAL PROPERTIES
k) Figure 12: Typical Physical Properties – Metric &amp; Imperial1
Property2
XL
SXL
Ultimate Tensile Strength3
MPa
ASTM D-412
psi
% Elongation - ASTM D-412
Young’s Modulus
MPa
(tensile)
psi
Poisson Ratio
Izod Impact -notched Joules/m
Avg. - ASTM D-256
ft-lb/in
Specific Gravity
Thermal
W/m-k
Conductivity
Btu/hr-ft-F
Thermal
KJ/kg-k @ 30&deg;C
Capacity
Btu/lbm-F @ 86&deg;F
Coefficient of Thermal Expansion
Strain
x 10-5 (&deg;C) or (&deg;F)
35
5000
70
850
123 000
~ 0.45
~ 150
~3
1.21
~ 0.25
~ 0.14
~1.5
~ 0.36
37.5
5450
150
605
88 000
~ 0.45
~ 500
~9
1.16
~ 0.25
~ 0.14
~1.5
~ 0.36
T &lt; 0&deg;C
0&deg;C &lt; T &lt; 30&deg;C
T &gt; 30&deg;C
T &lt; 32&deg;F
32&deg;F &lt; T &lt; 86&deg;F
T &gt; 86&deg;F
Volumetric Swell (%)@20&deg;C (68&deg;F)
-Water
-TL3G/Oil/Grease
Compression Set (%)
Ref. ASTM D395 method B
Coefficient of Friction
10.2
14.8
18.1
5.7
8.2
10.1
10.9
15.1
21.1
6.1
8.4
11.7
1.3
1.3
1.3
1.3
-
-
Dry static
dynamic
Wet static
dynamic
Flammability
- ASTM D-635-56T
Min. / Max.
Operating Temperature
Dry 5
Wet
Oil/Grease
0.35 - 0.45
0.30 – 0.40
0.30 – 0.40
0.20 – 0.25
SE 4
&deg;C
&deg;F
&deg;C
&deg;F
&deg;C
&deg;F
-60/107
-76/225
-7/60
20/140
/75
/167
0.25
0.10
0.25
0.10
–
–
–
–
0.35
0.20
0.35
0.20
SE
-60/107
-76/225
-7/60
20/140
/75
/167
HPSXL
COMPAC
Composite
(GM2401)
40
5800
70
925
134 000
~ 0.45
1.28
~ 0.25
~ 0.14
~ 1.5
~ 0.36
(-20&deg;C &lt; T &lt; 80&deg;C)
(-4&deg;F &lt; T &lt; 176&deg;F)
12 x 10-5 &deg;C or 6.7 x 10-5 &deg;F
37.5
5450
150
605
88 000
~ 0.45
~ 500
~9
1.16
~ 0.25
~ 0.14
~1.5
~ 0.36
17
2500
265
~ 0.45
sample
not broken
1.10
~ 0.25
~ 0.14
~1.5
~ 0.36
{
10.9
15.1
21.1
6.1
8.4
11.7
~10.2
~14.8
~18.1
~5.7
~8.2
~10.1
1.3
1.3
~1.3
-
-
27%
&lt; 200 Bar
&lt; 3000 psi
~0.35
0.28 – 0.35
0.30 – 0.40
0.25 – 0.35
&gt; 200 Bar
&gt; 3000 psi
0.09 – 0.15
0.07 – 0.12
0.08 – 0.15
0.06 – 0.12
SE
-60/107
-76/225
-7/60
20/140
0.25
0.10
0.25
0.10
–
–
–
–
0.35
0.20
0.35
0.20
SE
-60/107
-76/225
-7/60
20/140
/75
/167
0.40
0.15 – 0.20
SE
-7/60
20/140
Notes:
1
Appearance of ‘~’ is indicative of interpolated or estimated values based on in-house testing of this or similar materials.
2
All tests to develop the above data were done under carefully controlled conditions in our own laboratory to ensure the most accurate relative data
possible. Bear in mind that comparison of tensile strength is less meaningful for non-metallic materials compared with metals. This is especially true
of non-metallic bearings loaded in compression.
3
The Ultimate Tensile Strength (UTS) values are based on the mean value, for production batches over the last 10 years for XL and SXL &amp; GM2401
(5 years for HPSXL ) minus 2 standard deviations of the variable results.
4
SE — self extinguishing
5
Material used at dry temperatures exceeding 60&deg;C (140&deg;F) must be retained by suitable positive means. Please review these applications with
Thordon Engineering.
12
DESIGN GUIDE
Figure 13: Bearing Pressure
4) DESIGN GUIDE
a) Application Analysis
b) Bearing Pressure
c) Velocity
d) PVT Graphs
e) Length/Diameter (L/D) Ratio
f) Wall Thickness
g) Mating Surface
h) Fitting
i) Machining Tolerances
j) Minimizing Initial Installed Clearance
k) Selection Process
l) Problems and Causes of Bearing Failure
a) APPLICATION ANALYSIS
In order to perform any analysis of an application, all the
appropriate information must be reviewed and correctly
evaluated. The following list covers the general subject
headings which have been discussed in detail in previous
sections or will be discussed in this section.
• Operating Environment
(i) Temperature (ii) Abrasive or Clean
• Pressure
• Sliding Velocity
• Type of Lubrication
• Size
• Method of Retention
• Previous material used and problems associated
with it.
• Mating Surface
• Life Requirements
• Duty Cycle
• Initial Clearance Requirements
BEARING
PROJECTED AREA
WALL THICKNESS (1)
I.D
.
LEN
FIG. 11
GTH
normal operating load or a combination of static and
These factors all need to be analyzed in the grade
selection process as noted in sub-section 4 a).
Bearing
Pressure
=
Projected Area
=
Length x I.D.
c) VELOCITY
The sliding velocity or the peripheral shaft speed is
an important design factor. Velocity is an essential
consideration when evaluating frictional heat generation.
It is calculated by the following equation for
rotating shafts.
V =
V =
π dN (m/sec) or
60 x 1000
dN (m/sec)
19,100
π dN (fpm)
12
or .262 dN (fpm)
where
V = Sliding Velocity
d = Shaft Diameter (mm or in.)
N = RPM of the shaft
π = pi constant 3.1416
b) BEARING PRESSURE
d) PVT GRAPHS
by the projected or cross sectional area. The projected
area is determined by multiplying the inside diameter of
the bearing by the bearing length, as in Figure 13. The
use of inside diameter multiplied by bearing length is a
bearing industry norm for calculating the projected area
for bearing pressure. Dividing the load by the projected
area gives the approximate pressure. This assumes that
the pressure is uniform across the bearing area. In reality,
the pressure is greatest at the 6 o’clock position and
decreases in a parabolic curve to zero where the shaft
starts to have clearance with the bearing. It is therefore
running clearances to a minimum.
Any sliding bearing analysis is always based on three
factors. Pressure, Velocity and Time (PVT) are individual
factors that are impossible to separate when selecting
a bearing material because the heat generated is
proportional to all three as shown in the following
relationship:
H ~ PV&micro;T
where
H = Heat or Temperature Rise
P = Pressure
V = Velocity
&micro; = Coefficient of Friction
T = Time
13
DESIGN GUIDE
In order to evaluate an application, it is necessary to
know the duty cycle of the equipment. How long per day
does it run, i.e. 8 hours, 24 hours or stop and start? Is
there full rotation, which is normally specified in RPM, or
does it cycle or oscillate through a limited angle? Through
what angle and how frequently does movement occur and
how many hours a day (Duty Cycle)? These factors all play
a role in determining the amount of frictional heat that
will be generated under defined pressures.
However, if the frictional heat generated is removed
by a sufficient flow of cooling lubricant such as water,
oil or process liquid, Thordon bearings will perform
well at velocities far outside the limits shown on
the PVT graphs. Typical applications where this occurs
include marine propeller shaft and vertical pump
or turbine shaft bearings where a constant flow of
cool water is provided. The minimum recommended
cooling water flow rate is 0.15 litres/minute/mm
(1 US Gal/minute/inch) of shaft diameter.
The PVT graphs -Figures 14(a) to (f)- have been developed
by Thordon Bearings Inc. as a guide for the design
engineer in the selection of the correct grade of Thordon
for specific operating pressures, sliding velocities and
times. The curves have been developed using the pressure
step technique, where the material is tested at one
pressure under various velocities with the limiting factor
being bearing temperature. The arbitrarily imposed
temperature limit for all of the Thordon grades during the
tests was 82&deg;C (180&deg;F), measured at the outside diameter
of the bearing, except when tested in water. The limit in
water was set at 60&deg;C (140&deg;F) to avoid hydrolysis. When
the limiting temperature was reached during the test, the
test was stopped and the time recorded. The test sample
the test was repeated for another velocity. The tests were
conducted using bearings with a shape factor of 4.
To use the graphs, select the type of lubrication that
is closest to your application. Locate the sliding velocity
value for your application. Where the sliding velocity
makes contact with the curve closest to your pressure,
read the time required to reach the operational
temperature limit. If the time required for your
application is less than this value, then this application
will likely be suitable. If not, then either a different
Thordon grade needs to be selected, or improved
lubrication or cooling provided.
14
The PVT graphs for oil and water were developed using a
bath of oil or water with no liquid flow or cooling. If the
system can be designed to incorporate a forced flow of
cool lubricant instead of a bath, much of the frictional
heat will be dissipated by the flow of lubricant. Once the
bearing is operating under hydrodynamic conditions, no
additional frictional heat is developed as the speed is
increased, except for a slight increase in frictional drag
of the lubricant. This increase is so low that it does not
affect the bearing operation.
Under the forced cool lubricant flow conditions, the
limits on the graphs are not applicable. The stern tube
of a ship using water or oil lubrication is typical of
this situation.
The PVT graphs are provided as a guide only. Thordon
has been successfully specified in many applications with
PVT’s falling outside the range on the graphs. For example,
Thordon SXL has been incorporated into a number of
vertical pump designs where it runs dry for periods of
over a minute at velocities higher than indicated on
the curves.
NOTE 1: For guidance on potential applications that fall outside the
PVT graphs contact your Thordon distributor or Thordon Bearings Inc.
NOTE 2: PV values are given by many non-metallic material
manufacturers and are often published with several incorrect
assumptions. The first is that the individual P and V values have
little importance, as long as they are with the product value range.
The second, and perhaps the most dangerous assumption is the
limited amount of test time used to develop the P and V values.
No formal consideration is given to the time factor. The Thordon
PVT graphs illustrated in Figure 14 show that frictional heat takes
time to be generated.
NOTE 3: These graphs are based on laboratory results. Actual results
in applications may vary.
NOTE 4: These guideline values are supplied for reference only.
PV limits for any material vary with different combinations of pressure
and velocity as well as with other test conditions.
100
250
100
(1)
150
NOTE: These tests were conducted using a bearing with a shape factor of 4.
NOTE: These tests were conducted using a bearing with a shape factor of 4.
200
(1) 53.3 psi (0.37 MPa)
(2) 106 psi (0.73 MPa)
(3) 250 psi (1.72 MPa)
CONDITION –– DRY
FIG. 12(b)
50
1.0
THORDON SXL
0.8
FIG. 12(a)
25
(3)
(2)
0.6
SURFACE VELOCITY (m/s)
0.4
SURFACE VELOCITY (fpm)
0
0.2
SURFACE VELOCITY (fpm)
.1
.1
200
.2
.2
150
.4
.4
50
.6
.6
25
.8
2
4
6
8
10
20
.8
(1)
(1) 53.3 psi (0.37 MPa)
(2) 71.1 psi (0.50 MPa)
(3) 106 psi (0.73 MPa)
(4) 240 psi (1.65 MPa)
CONDITION –– DRY
1
0
(4)
(3)
(2)
100
0
1
2
4
6
8
10
20
RUNNING TIME (hours)
THORDON XL
1.4
40
1.2
40
1.0
60
0.8
60
0.6
SURFACE VELOCITY (m/s)
0.4
80
0.2
RUNNING TIME (hours)
1.2
Figure 14b: PVT Graph for SXL – Lubrication: Dry
LUBRICATION: DRY
80
100
0
Figure 14a: PVT Graph for XL – Lubrication: Dry
250
1.4
DESIGN GUIDE
15
50
500
600
700
100
200
300
400
(1)
NOTE: These tests were conducted using a bearing with a shape factor of 4.
NOTE: These tests were conducted using a bearing with a shape factor of 4.
FIG. 12(d)
50
(3)
(2)
3.0
500
600
(1) 240 psi (1.65 MPa)
(2) 550 psi (3.79 MPa)
(3) 750 psi (5.17 MPa)
FIG. 12(c)
0
THORDON SXL
2.5
CONDITION –– WATER BATH
2.0
These tests were conducted with no flow, no circulation.
1.5
SURFACE VELOCITY (m/s)
1.0
SURFACE VELOCITY (fpm)
.1
400
.1
300
.2
.2
0.5
SURFACE VELOCITY (fpm)
.4
.4
200
.6
.6
2
4
6
8
10
20
.8
100
(2)
(1)
(1) 106 psi (0.73 MPa)
(2) 240 psi (1.65 MPa)
(3) 550 psi (3.79 MPa)
These tests were conducted with no flow, no circulation.
CONDITION –– WATER BATH
.8
0
0
100
1
(3)
3.5
1
2
4
6
8
10
20
THORDON XL
3.0
40
2.5
40
2.0
60
1.5
60
1.0
SURFACE VELOCITY (m/s)
80
0.5
80
0
100
RUNNING TIME (hours)
16
RUNNING TIME (hours)
700
3.5
Figure 14d: PVT Graph for SXL – Lubrication: Water Bath
LUBRICATION: WATER BATH
Figure 14c: PVT Graph for XL – Lubrication: Water Bath
DESIGN GUIDE
RUNNING TIME (hours)
50
500
600
700
200
300
(1)
NOTE: These tests were conducted using a bearing with a shape factor of 4.
NOTE: These tests were conducted using a bearing with a shape factor of 4.
1.5
400
500
600
(1) 250 psi (1.72 MPa)
(2) 550 psi (3.79 MPa)
(3) 950 psi (6.55 MPa)
CONDITION –– GREASED
FIG. 12(f)
100
1.25
THORDON XL &amp; SXL
1.0
FIG. 12(e)
50
(3)
(2)
.75
SURFACE VELOCITY (m/s)
.50
SURFACE VELOCITY (fpm)
0
.25
SURFACE VELOCITY (fpm)
.1
400
.1
300
.2
.2
200
.4
.4
100
.6
.6
0
.8
.8
2
4
6
8
10
20
1
(1)
(1) 550 psi (3.79 MPa)
(2) 750 psi (5.17 MPa)
(3) 950 psi (6.55 MPa)
CONDITION –– OIL BATH
1
2
4
6
8
10
20
(3)
(2)
0
100
RUNNING TIME (hours)
THORDON XL &amp; SXL
3.5
40
3.0
40
2.5
60
2.0
60
1.5
SURFACE VELOCITY (m/s)
1.0
80
0.5
80
100
0
700
1.75
Figure 14e: PVT Graph for XL &amp; SXL – Lubrication:
Oil Bath
Figure 14f: PVT Graph for XL &amp; SXL – Lubrication: Grease
LUBRICATION: OIL BATH / GREASED
DESIGN GUIDE
17
DESIGN GUIDE
The L/D ratio for a typical industrial sleeve bearing
varies from 1:1 to 1.5:1. This is an optimum proportion
permitting ease of alignment in the assembly.
In water lubricated propeller shaft bearing applications,
the L/D ratio has historically been 4:1 in order to keep
the bearing pressure low, i.e. 0.25 MPa (36.25 psi).
However, because of the overhung load of the propeller,
the pressure distribution tends to be highest nearer
the propeller and almost zero at the forward end. In
operation, the high L/D ratio tends to create higher
friction or drag on the shaft. This is because the forward
part of the bearing is not supporting the shaft and creates
unnecessary shearing of the water. There may even be
contact between the shaft and bearing at the top of
the bearing at the forward end. A 2:1 L/D ratio Thordon
propeller shaft bearing was tested under the same
conditions as the 4:1 and was found to generate less
frictional force. The results of these tests in conjunction
with encouragement from the marine Classification
Societies resulted in the development of the Thordon
COMPAC bearing system.
is uniform, higher L/D ratios will reduce the pressure
and improve the life of the bearings. Alignment is more
difficult, but if the pressure is high, an increase in the
L/D ratio may be necessary. For COMPAC propeller shaft
bearings, the L/D ratio should not be more than 3:1.
This limit is established because of concerns about the
supply of adequate cooling water to very long bearings
rotating at relatively high speeds.
For high pressure limited rotation applications, Thordon
HPSXL TRAXL or ThorPlas&reg; bearings should be considered.
f) WALL THICKNESS
Due to the elastomeric nature of the material, a Thordon
bearing must be supported along its entire length.
An unsupported bearing will carry virtually no load.
If wall thickness can be specified in the design, it is
generally preferable to use a thinner wall. The overall
clearances and tolerances can be reduced, heat dissipation
is improved and the maximum permissible load is greater.
There are some applications, however, such as those with
low frequency impact loads where the cushioning effect
of a thicker wall bearing will improve performance. Please
contact your Thordon distributor or Thordon Bearings
for further guidance on wall thickness, if required. Given
application details, Thordon Bearings can recommend
an optimum wall thickness. The Thordon Bearing Sizing
Calculation program can also provide this information.
Minimum Recommended Wall Thickness Guide
for Interference Fitting
The minimum recommended wall thickness of a Thordon
bearing is specified in Figure 15. The values shown are
based on the interface pressure between the bearing
and the housing. Increasing either the wall thickness
or the amount of interference will increase the interface
pressure. In both grooved and ungrooved bearings, the
thickness of the bearing wall that forms a continuous
layer in the housing is the only material considered for
interference fitting purposes. With grooved bearings,
the minimum wall thickness will be greater than that
of an ungrooved bearing by the amount of the depth
of the groove as only the thickness behind the groove
is considered when calculating the interface pressure.
For Thordon Composite bearings, only the thickness of
the yellow outer shell material should be considered
when determining the minimum wall thickness. The
bearing running surface material (GM2401) is too soft
to contribute to the interface pressure.
In an application where Thordon is being specified
as a replacement bearing, the existing configuration
of the equipment usually governs the wall thickness
of the bearing.
The degree of Permissible Wear Down before a
bearing is ‘worn out’ is also a factor in determining
wall thickness. Maximum allowable clearance and
other external factors also enter into this consideration.
For grooved bearings, maximum allowable wear should
be less than the groove depth.
18
MINIMUM RECOMMENDED WALL THICKNESS GUIDE
FOR INTERFERENCE FITTING OF THORDON BEARINGS
WALL THICKNESS (mm)
0
40
10
20
30
40
50
60
1000
800
30
SHAFT DIAMETER (inches)
If the wall thickness of the Thordon bearing is going to
be excessive, the bearing can be used in conjunction
with a metal sleeve in the housing or a liner on the shaft.
Either of these methods will allow a reduction in the wall
thickness of the bearing. If a shaft liner is used, a further
benefit results - as the effective diameter of the shaft and
the I.D. of the bearing increase, the pressure decreases.
Figure 15: Wall Thickness Guide
600
20
400
SHAFT DIAMETER (mm)
e) LENGTH/DIAMETER (L/D) RATIO
10
200
0
0.0
0
0.5
1.0
1.5
2.0
2.5
WALL THICKNESS (inches)
NOTE: For grooved bearing, wall thickness is measured from bottom of groove to the ID.
DESIGN GUIDE
If a Thordon bearing is replacing another bearing and the
wall thickness will be below the recommended minimum
there are two options. The bearing can be bonded in, or
the interference can be increased to raise the amount of
your Thordon distributor or Thordon Bearings for further
guidance if the level of interference is to be increased.
NOTE 1: The above information applies to Thordon XL, SXL and COMPAC.
It does not apply to HPSXL. Thordon HPSXL is not recommended for
interference fitting. It should be bonded.
g) LUBRICATION GROOVES
For applications involving a flow of liquid across the
bearing surface, such as vertical pump or propeller shaft
bearings, lubrication grooves are machined or moulded
into the bearing to aid in the flow of lubricant through
the bearing. The grooves also provide a channel to allow
abrasives to pass. The number of grooves as well as
their depth and width change with the size of the
bearing, its configuration and the available wall thickness.
Water grooves are typically 7mm (0.27”) deep for shaft
diameters of 400mm (16”) or larger, but should not
be more than half of the wall thickness. The width of
the groove is typically the same as the depth, but can
be increased when grooves are very shallow to ensure
sufficient water flow. The Thordon Bearing Sizing
Calculation Program provides details of depth and number
of grooves for any grooved bearing application, based
Thordon Bearings for further information on
lubrication grooves.
h) MATING SURFACE
Most common metallic mating surfaces will perform well
when used in conjunction with Thordon bearings. Figure
16 indicates the hardness of commonly used mating
materials. If corrosion is not a problem, carbon steel is
commonly used, but if corrosion is a concern, such as a
water lubricated propeller shaft bearing, then a bronze
shaft liner should be used. Common bronzes that work
well include Gunmetal (88% Cu, 10% Sn and 2% Zn)
or 70-30 Copper Nickel. Nickel Aluminum Bronze is not
recommended because experience has show that it
can lead to high wear rates. Aluminum and titanium
are also not recommended.
Figure 16: Hardness of Commonly Used Mating Material1
Material
Rockwell C
Hardness
Rockwell B
Brinell5
Remarks
(16) 4
95
(205)
Annealed
30.5
(1)
26 to 43
31
33 to 44
(105)
82
(103 to 113)
(106)
(108 to 114)
290
(156)
(258 to 400)
(294)
(311 to 409)
Annealed
Oil quenched from 1010&deg;C &amp; Tempered
Annealed
Water quenched from 1038&deg;C &amp; Tempered
N/A
81
(153)
Annealed
N/A
N/A
70 to 95
N/A
N/A
70 to 85
N/A
(21)
N/A
&gt; 60
74
98
75
N/A
(135)
(228)
(137)
&gt; 654
2
Stainless Steel
316
Stainless Steel
Duplex 2205 (S 31803)
Stainless Steel
S41000
Stainless Steel
S17400
Stainless Steel
S30400
Gunmetal (G1) 3
C90500
C92200
70/30 Copper –Nickel
C96600
Inconel 625
Inconel 600
Nickel-Chrome-Boron (NiCrB)
Annealed
Annealed
Surface coating
Notes:
1
The purpose of listed hardness value is for quick hand-on reference. Refer to textbook for more details if necessary.
2
See “Stainless Steel, ASM Specialty Handbook” edited by J.R. Davis, 1994, ISBN:0-87170-503-6 for stainless steel details.
3
See “Standards Handbook”, Cast Copper and Copper Alloy Products, published 1996 by Copper Development Association Inc. 260 Madison Avenue,
New York, NY10016 for bronze details.
4
The number in brackets was converted from the unbracketed using conversion tables and is for comparison purposes only.
5
BRINELL scale used in this table is BHN 3000kg.
19
DESIGN GUIDE
Stainless steel is also widely used as a shaft liner working
with a Thordon bearing. If abrasion is present, softer
stainless grades like 304 should be avoided. Similarly,
the softer grades of Aquamet shafting should be avoided
if the shafts will be exposed to significant abrasion.
Harder grades of stainless steel, or Inconel 625 are
preferred. In lieu of a liner, some manufacturers use spiral
welded stainless steel or Inconel 625 over the whole
length of the shaft, or in way of the journals.
In a heavily abrasive journal bearing application, the
theoretical optimum mating surface is the hardest
practical surface on the shaft in conjunction with a
durable compliant bearing material. For severe abrasives,
a Thordon Composite bearing and a mating surface
with a hardness of at least 40 Rockwell C is recommended.
Thordon grades cause minimal shaft wear. In general,
softer bearing materials such as Thordon tend to wear
the shaft less and exhibit less combined bearing and
shaft wear. The harder materials are more suitable for
abrasive conditions.
The hardest shaft and softest bearing materials are the
extremes to achieve minimum combined wear in a severe
abrasive environment. If the shaft were changed to a
softer material or if the bearing were changed to a harder
material, the combined wear would increase. Should
the environment contain fewer abrasives, then the need
to have the hardest shaft material or softest bearing
material would decrease. Other factors such as low
friction requirements may then become significant in
bearing selection.
In a clean environment with a lubricant (which only
occurs in theory) any combination will do. However, the
old principle of a bearing softer than the mating shaft is
always a good guide. Running similar materials together
should be avoided. Thordon should not be run against
a Thordon shaft liner.
The Surface Finish of the mating shaft should be as
smooth as practical to limit the initial bedding-in wear.
Thordon testing has shown that less frictional heat is
generated with a smoother shaft, increasing the PVT
limit. Thordon will perform satisfactorily with a normal
machined finish on the shaft. For optimum performance,
a final machined mating surface finish of 0.4 to 0.8
micro-metres (16 to 32 micro-inches) Ra is recommended.
Mating shaft surface finishes up to 1.6 micro-metres
(63 micro-inches) Ra will perform satisfactorily.
i) FITTING
Thordon XL, SXL, COMPAC and Composite bearings are
usually fitted using an interference fit. Installation is
quick and easy, especially when freeze fitting is used.
Thordon bearings can also be bonded in place. Bonding,
using a Thordon approved adhesive, is appropriate in
the following circumstances:
20
• where a thin walled bearing is used and retention
force is not sufficient for an interference fit
• when the housing I.D. is not machined, or when
it does not provide adequate support along the
full length of the bearing.
• when bearings are subjected to high temperatures
that may cause them to “stress relieve” and lose
the retention force of an interference fit.
• when Thordon HPSXL is used.
• when the housing is not round or is damaged
by corrosion, etc.
The final dimensions of a Thordon bearing will depend on
how it is to be fitted. The selection of the best method of
fitting is extremely important and is dependent on
application requirements.
An interference fit is sufficient to prevent bearing rotation
under normal operating conditions, but a forward stop
and bolted end keeper ring are required to ensure that
axial movement of the bearing does not occur. The
keeper rings must be of adequate size and have an
inside diameter approximately 3 mm (1/8”) larger than
the groove diameter. Stops and keeper rings are not
mandatory when a bearing is bonded in place but
are recommended in critical applications as a safety
precaution. In cases where the orientation of the bearing
is critical such as off-centre bored bearings or COMPAC, it
is recommended that an anti-rotation device be fitted.
(i) Interference
Most applications can be accomplished using an
interference fit assuming all the relevant design factors
are taken into account. It is necessary, however, that
the L/D ratio of the bearing be at least 0.5:1. Practical
experience has shown that small bearings can be easily
pressed into the housing, while larger bearings fit easier
when they are shrunk using dry ice or liquid nitrogen. The
housing should never be heated to facilitate fitting, nor
should grease or oil be used to assist when press fitting.
In cases where the bearing is being installed with
an interference fit as in Figure 17, the effect of the
interference on the bearing inside diameter must also
be considered. This effect, known as bore closure, is
explained in Section 5 - Application Design.
All interference fit bearings that are fully machined before
installation are subject to a build up of tolerances which
can create additional installed clearance. For example,
when a bearing is designed with minimum clearance, its
actual clearance will be dependent on the accumulated
machining tolerances of the bearing wall thickness, plus
tolerances on the shaft and housing. This tolerance build
up can be reduced by machining only the O.D. of the
bearing prior to fitting and then machining the I.D. up
to a maximum of 5% of the wall thickness after it is
DESIGN GUIDE
INTERFERENCE
FIT PARAMETERS
Figure 17: Interference
Fit Parameters
FORCE
PRESS
IN FORCE
PRESSIN
1.
2.
Housing
Shaft
3.
Where:
Is Interference.
Where:1. 1.
is interference,
2. is Bore Closure, 3. is Installed Running Clearance.
2. Is Bore Closure.
3. Is Installed Running Clearance.
Note: Minimum Installed Clearance = Running Clearance
Minimum
Installed
Clearance
=
+ Thermal
Expansion
Allowance
(if applicable)
Clearance
Running
+ Water
Absorption Allowance (if applicable)
Note:
+ Thermal Expansion Allowance (if applicable)
+ Water Absorption Allowance (if applicable)
installed. This will eliminate the tolerance build up
associated with bore closure, bearing wall and housing
I.D. Bore Closure is the most variable of the factors
affecting Thordon bearing installed dimensions. There can
be situations where, in practice, the bore closure varies
from that predicted by our tests, and can result in
additional clearances. If it is not possible to machine the
bearing I.D. after installation, a test bearing can be fitted
into a machined “dummy” housing to determine the exact
bore closure for that application. The finish on the I.D. of
the “dummy” housing should be the same as that on the
actual housing. Corresponding adjustments if required, can
then be made. Alternatively, bearings can be machined in
the “dummy” housing, removed and fitted into the actual
housing. This approach is sometimes used for vertical
pump or turbine bearings where there is a requirement
to keep the initial installed clearance as small as possible.
easily installed (approximately 5 to 30 minutes depending
on the surface area of the bearing). If dry ice is used
as the cooling medium it should be supplied in pellets
or broken into small pieces, if supplied in block form.
The dry ice must be packed tightly around the O.D. of
the bearing with some clearance around the I.D. of the
bearing, making contact with both the inside and outside
surfaces. After 3 hours packed in dry ice the bearing
dimensions can be checked to see if the bearing has
shrunk sufficiently to allow easy installation. If not,
the bearing should be re-packed for another hour.
CAUTION: Use of liquid nitrogen or significant quantities
of dry ice in closed or poorly ventilated areas should be
avoided. The boiled off gases tend to displace the existing
oxygen and can be fatal.
The approximate amount of shrinkage that can be
expected can be estimated as follows:
- Each 10&deg;C decrease in temperature will result in an
approximate decrease in diameter of 0.0014 mm/mm
of diameter (Each 10&deg;F decrease in temperature will
result in an approximate decrease in diameter of
0.0008 in./in. of diameter).
(iii)Bonding
As indicated previously, bonding is an acceptable
alternative to interference fit in selected circumstances.
The thickness of the layer of adhesive must be considered
when dimensioning the O.D. of the bearing. When
bearings are bonded into housings, there is no bore
closure effect on the bearing I.D. (see Figure 18).
To hold the accumulation of tolerances to a minimum, the
bearing should be machined on the O.D. and then bonded
into the housing. The I.D. should then be machined. This
method is used in pump applications where the impeller
clearance must be held to a minimum.
BOND
FITBond
PARAMETERS
Figure 18:
Fit Parameters
(ii) Freeze Fitting
Freeze fitting is the easiest way to install Thordon
bearings which have been designed with an interference
fit. Thordon contracts significantly when cooled, because
of its high coefficient of thermal contraction/expansion,
thus facilitating easy fitting without expensive jacking
or other equipment. Liquid nitrogen is the optimum
cooling agent but dry ice can also be used for most
installations if liquid nitrogen is not available. When
freeze fitting Composite Bearings, dry ice should be
used and not liquid nitrogen.
Liquid nitrogen should only be used in a tight container
to prevent leakage. The bearing should be completely
immersed in, or evenly coated with, liquid nitrogen. When
vapour stops boiling off the liquid nitrogen the bearing
has reached a temperature of -196&deg;C (-320&deg;F) and can be
1.
2.
Housing
Shaft
Where:
Where:1. 1.
Is Bond
Thickness.
is Bond
Thickness,
2. is Installed Running Clearance.
2. Is Installed Running Clearance.
Note: Minimum Installed Clearance = Running Clearance
Note: Minimum
Installed
Clearance
= (if applicable)
+ Thermal
Expansion
Allowance
Running Clearance
+ Water Absorption Allowance (if applicable)
+ Thermal Expansion Allowance (if applicable)
+ Water Absorption Allowance (if applicable)
21
DESIGN GUIDE
To ensure good results are achieved, the procedures
for bonding using Thordon approved adhesives must
be followed, as outlined in Appendix 1.
Bonding should be done at a consistent temperature
throughout the adhesive curing process. Temperature
variations during curing can have a negative effect on
the bond integrity. Combining freezing and bonding does
not work well because the moisture/frost on the frozen
bearing will have a significant negative impact on the
bond strength.
(iv) Bearing Housing
The housing into which a Thordon bearing is to be
installed must be round, aligned, and not tapered or
bell-mouthed. The maximum allowable housing ovality
is 1/3 the initial (normal) designed running clearance.
The housing must also provide support to the Thordon
bearing along its full length. Gaps in the housing or other
abnormalities must be corrected by machining, installing
a sleeve, bonding the bearing (for gaps up to 3 mm
(0.125”) or chocking with a Thordon approved chocking
compound.
If the housing is misaligned, or if there is a need for
slope boring, then the misalignment or slope should
be corrected in the housing. Offset boring of Thordon
bearings after fitting is not recommended because of the
possible adverse effect this could have on the interference
hoop stresses. Alternatives are to align a machined
bearing and then bond or chock it in place, or to align
a “dummy” bearing, pour chocking compound around
the “dummy” bearing and then remove the “dummy”
bearing leaving a round aligned housing of chocking
material into which a Thordon bearing can be installed
using a press or freeze fit.
j) MACHINING TOLERANCES
Thordon, a non-metallic material, cannot be machined
to the same tight tolerances as bronze or other rigid
materials. At the same time, metallic tolerances are not
necessary to obtain optimum performance. The standard
Thordon machining tolerances for O.D., I.D., W.T. (Wall
Thickness) and Length are as follows:
Bearings up to 330mm (13.00”)
O.D. +0.13mm, -0.00mm (+0.005”, -0.000”)
I.D. +0.13mm, -0.00mm (+0.005”, -0.000”)
Bearings between 330 and 530mm (13.00” and 21.00”)
O.D. +0.18mm, -0.00mm (+0.007”, -0.000”)
Wall thickness (W.T.)
+0.00mm, -0.13mm (+0.000”, -0.005”)
I.D.(Composite only)
+0.18mm, -0.00mm (+0.007”, -0.000”)
22
Bearings over 530mm (21.00”)
O.D. +0.25mm, -0.00mm (+0.010”, -0.000”)
W.T. +0.00mm, -0.13mm (+0.000”, -0.005”)
I.D. (Composite only)
+0.25mm, -0.00mm (+0.010”, -0.000”)
Bearing Length Tolerance:
For bearings shorter than 500mm (20”) long
+0.00mm, -0.50mm
(+0.000”, -0.020”)
For bearings longer than 500mm (20”) long
+0.00mm, -1.00mm
(+0.000”, -0.040”)
NOTE 1: For Thordon XL, SXL and COMPAC bearings over 330 mm (13&quot;),
machined I.D. tolerance should be controlled by controlling the wall
thickness of the bearing. For Composite bearings over 330 mm (13&quot;)
only, the actual I.D. of the bearing should be controlled.
NOTE 2: If the wall thickness is less than 25mm (1”) then there may be
restrictions as to the length of bearing that can be properly machined.
Consult Thordon Bearings for details.
NOTE 3: If an application requires tolerances that are tighter than those
Thordon Bearings for guidance.
k) MINIMIZING INITIAL
INSTALLED CLEARANCE
Initial installed clearance for Thordon bearings is usually
larger than final running clearance, mainly because the
initial clearance includes absorption and thermal expansion
allowances. These allowances will disappear during
operation of the equipment, but this will take time.
In some applications, there is a requirement to keep the
initial installed clearance as small as possible. A typical
example would be a vertical pump bearing. Final running
clearance may be acceptable, but when absorption
allowance, thermal expansion and tolerance build-up are
considered, the accumulated initial clearance may be
beyond design requirements. In such cases it is necessary
to consider ways to reduce the initial clearance. There are
several options:
1) Thinner bearing - Absorption and thermal expansion
both vary according to the wall thickness of the
bearing. By reducing the wall thickness, the
allowances for these factors become smaller, so
the initial clearance is reduced. Reducing the wall
thickness is usually accomplished by reducing
the housing diameter. The Thordon Bearing Sizing
Calculation program can be useful in this exercise –
it calculates “Minimum Installed Clearance”. It can
be used to determine what wall thickness will yield
the required initial clearance. The wall may become
too thin for an interference fit, so bonding may
be required.
DESIGN GUIDE
2) Minimize bore closure variations – The bore closure
calculation (effect of interference on the I.D. of the
bearing) is the least precise aspect of the Thordon
dimension calculations. Actual bore closure will
depend on a number of factors including machined
finish on the bearing and housing. There are several
ways to minimize variations in bore closure:
a) Reducing the length/diameter ratio of the
bearing will reduce variations in bore closure
over the length.
b) Final machining of the bearing bore after it
is installed. Machining after fitting into the
housing eliminates the effect of bore closure
because it has already happened. It also
eliminates the effect of tolerance build-up on
the bearing wall. This method however removes
stressed material that is developing the “grip” of
the bearing within its housing so only minimum
material must be removed.
• For ungrooved bearings, this machining stage
must not remove more than 5% of the wall
thickness.
• For grooved bearings, it is not as important
because the bore material is much less stressed.
However, machining should be limited to 10% of
the wall thickness or 25% of the groove depth,
whichever is less. Lubrication grooves must
always be machined before fitting the bearing
into the housing.
c) Fitting the bearing into a dummy housing before
machining the I.D. This method is a variation
of “b” above which can be used when it is not
practical to install the bearing in its final housing
for I.D. machining. The dummy housing should
have the exact dimensions and machining finish
as the final housing. This method is less precise
because it does not eliminate machining tolerance
variations on the housing. The same restrictions
on the amount of material that can be removed
mentioned in “b” above still apply.
l) SELECTION PROCESS
In any bearing application the primary consideration
is to ensure that the frictional heat developed in the
sliding action is either absorbed and dissipated by the
surrounding mechanism or that it is conducted away by
a flow of lubricant or coolant. There must be a balance
in the system where temperature equilibrium is reached,
and this must be below the temperature limit of the
material. If not, bearing failure will result.
The secondary consideration is the type of environment
that the bearing is operating in, e.g. very abrasive or
clean, as this will affect material selection.
NOTE: The General Material Selection Guide for Industrial Applications
(Figure 19) has been compiled to select the correct Thordon grade
for various application parameters, and should be used in conjunction
with the PVT graphs.
The Material Selection Guide does not consider any heat generation.
If the peripheral velocity is high enough to generate frictional heat,
then the maximum pressure will be significantly less. For example,
in marine propeller shafts with Thordon COMPAC, SXL and XL shaft
bearings, maximum pressure is limited to 0.6 MPa (87 psi).
For high pressure applications where the frictional heat
generated is not a factor due to either oscillating motion
or very slow speeds, the bearing needs to be designed
with a very high shape factor, e.g. above 100, as in the
Thordon HPSXL TRAXL bearing.
Thordon XL (Black) is used in a variety of industrial
and marine applications.
• low coefficient of friction (typically 0.20-0.25)
• high resistance to abrasion in dry applications
Thordon SXL (Off-White) has superior dry running
capability, a lower coefficient of friction and similar
abrasion resistance compared to XL.
• lower coefficient of friction (typically 0.10-0.20)
than XL
• higher dry PV (Pressure Velocity) rating than XL
• higher resistance to abrasion than XL in wet
applications; good abrasion resistance operating dry
• dry start-up capability as a vertical pump bearing
NOTE: When SXL is used in vertical pumps where dry startup is a
consideration, consult with Thordon Bearings regarding bearing design.
Thordon will recommend a maximum dry running time based on the
peripheral velocity of the shaft and the load on the bearing.
Thordon COMPAC (Orange) is a high performance grade
of Thordon that is used in open water lubricated propeller
shaft bearing systems. Specially formulated with a low
coefficient of friction to reduce startup friction and reduce
stick-slip, COMPAC’s unique configuration is designed to
promote early formation of a hydrodynamic film at lower
shaft rpm.
The COMPAC bearing system is Class-approved for 2:1 L/D
ratios. COMPAC’s design properties are quite similar to SXL.
Thordon Composite (Yellow shell, Black wear surface
is GM2401) is a two-component marine and pump
23
DESIGN GUIDE
bearing formulated specifically for use in very abrasive
environments.
• used in rotating applications in abrasive water
conditions such as pump and dredge bearings
• outstanding abrasion resistance - two or more
times that of rubber
• significantly lower coefficient of friction than rubber
• higher resilience and stiffness than rubber
• available with either yellow polymer or metal
bearing shells
Thordon HPSXL (Grey) is designed for higher pressure
applications, either as a homogeneous material or as
the bearing component in HPSXL TRAXL bearings (HPSXL
bonded in a metallic shell).
• maximum dynamic working pressure to 15.0 MPa
(2175 psi) in limited motion
• HPSXL TRAXL has maximum dynamic working pressure
to 55.0 MPa (8000 psi) in limited motion
• lowest coefficient of friction (typically 0.06-0.12)
• moderately abrasion resistant (lower abrasion
resistance than XL or SXL)
ThorPlas&reg; (Blue) is a non elastomeric material developed
by Thordon specifically as a homogeneous high pressure
bearing.
• maximum dynamic working pressure to 31.0 MPa
(4500 psi)
• low coefficient of friction (typically 0.10-0.17)
• very low wear in non-abrasive environments
• reasonable abrasion resistance - less than Thordon
elastomer grades, but better than bronze, epoxy
phenolics and many other non-metallic bearing
materials
ThorPlas&reg; is outside the scope of this manual.
distributor or Thordon Bearings.
Figure 19: General Material Selection Guide for Industrial Applications
Lubrication/
Operating Pressure
HHHHH
HHHH
Dry (sealed or minimal abrasives)
0-10 MPa (0-1450 psi)
10-15 MPa (1450-2175 psi)
15-31 MPa (2175-4500 psi)
31-55 MPa (4500-8000 psi)
SXL
HPSXL
HPSXL TRAXL
HPSXL TRAXL
ThorPlas&reg;
ThorPlas&reg;
ThorPlas&reg;
XL
SXL
HPSXL
ThorPlas&reg;
SXL
ThorPlas&reg;
ThorPlas&reg;
SXL
HPSXL
HPSXL TRAXL
HPSXL TRAXL
ThorPlas&reg;
ThorPlas&reg;
ThorPlas&reg;
GM2401
SXL
HPSXL
ThorPlas&reg;
SXL
ThorPlas&reg;
ThorPlas&reg;
Dry (abrasives present)
0-5.5 MPa (0-800 psi)
5.5-10 MPa (800-1450 psi)
10-15 MPa (1450-2175 psi)
15-31 MPa (2175-4500 psi)
Wet (sealed or minimal abrasives)
0-10 MPa (0-1450 psi)
10-15 MPa (1450-2175 psi)
15-31 MPa (2175-4500 psi)
31-55 MPa (4500-8000 psi)
Wet (abrasives present)
0-3 MPa (0-500 psi)
3-10 MPa (500-1450 psi)
10-15 MPa (1450-2175 psi)
15-31 MPa (2175-4500 psi)
HHH
ThorPlas&reg;
ThorPlas&reg;
Note:
The maximum pressures given for the various products are based on maximum dynamic working pressures for intermittent, limited motion. For
applications involving continuous rotary motion, PV limits of the materials will significantly reduce the maximum allowable pressures stated above.
This is a general guide for technical reference only. Other critical applications that are close to pressure or temperature limits, or subjected
to non-standard environments should also be reviewed and approved by Thordon Bearings.
24
DESIGN GUIDE
m) PROBLEMS &amp; CAUSES OF BEARING FAILURE
PROBLEM
CAUSE
SOLUTION
A) A bearing becomes loose in the
housing when subjected to a quick
reduction in temperature, even
when it is designed to operate at
that temperature.
When a bearing is installed with an
interference fit and then subjected to
a quick reduction in temperature, it
contracts faster than the material’s
ability to recover its interference fit.
When Thordon bearings are likely to
be subjected to this type of “Thermal
Shock”, the bearing should be bonded
into the housing and mechanically
retained.
B) A bearing becomes loose in the
housing when subjected to long
periods when the temperature is
greater than 60&deg;C (140&deg;F) for XL,
SXL, COMPAC and Composite
(GM2401).
The material has stress relieved itself
and adequate interference fit is no
longer present. When the temperature
is then reduced, the bearing will
shrink and come loose in the housing.
The bearing should be bonded into
the housing and mechanically
retained.
C) A bearing ‘walks’ or moves axially
out of the housing.
This normally occurs where the
pressure along the length of the
bearing is not uniform and cyclic,
and the component of forces produces
Ensure that the bearing is retained
axially with a keeper ring, or step
in the housing or that the bearing
is bonded into the housing.
D) A bearing seizes onto the shaft
causing interface melting.
Either insufficient clearance was
allowed or the combined PVT value
is too high.
Ensure that the correct clearance
is calculated allowing for running
clearance, water swell and thermal
expansion where applicable. Also
ensure that the correct bore closure
allowance is used for bearings
installed with an interference fit.
Check the PVT requirements to see
if auxiliary lubricant or coolant
is required.
E) A water lubricated bearing wipes
and takes on a glazed appearance
either covering the whole inside
diameter or only in the loaded
area. The bearing may have a
crazed or cracked appearance.
The bearing has been operating in
water at elevated temperatures, i.e.
over 60&deg;C (140&deg;F) or in steam. The
bearing has failed due to hydrolysis,
causing a softening or cracking of the
material.
Provide a cool water flush to the
bearing and do not use steam for
cleaning or flushing the bearing.
F) The bearing material separates as if
it has delaminated. The separation
takes place half way through the
wall thickness.
Internal heat build-up from high
caused the material to fail from
hysteresis.
The wall thickness of the bearing must
be reduced to limit deflection and
reduce the recovery time between
impacts. Review Thordon PVT Charts.
G) A bearing shows signs of having
softened – bulges on the ends of
the bearing or material flows into
the grooves.
The bearing does not have enough
lubrication to keep it cool. Frictional
heat generation is greater than what
can be dissipated through the
lubricant.
Improve lubrication flow:
– for water lubricated bearings ensure
that the flow is adequate and that the
water is cool.
- for other lubrication ensure that
there is sufficient lubricant and
adequate facilities for keeping it cool.
25
DESIGN GUIDE
m) PROBLEMS &amp; CAUSES OF BEARING FAILURE continued...
PROBLEM
CAUSE
SOLUTION
wears quickly and shows signs of
melting.
Check load on bearing relative to
pressure limits for Thordon Bearings
as indicated in Figure 19.
I) A water lubricated bearing wears
more rapidly than expected
and shaft liner is covered with
a white coating.
The white powder is cathodic chalk
that can be deposited on the shaft
liner when the ship’s cathodic
protection system is stronger than
necessary.
Clean shaft liner and reduce level of
cathodic protection. If ship spends
a lot of time in one specific port,
investigate cathodic protection of
the dock that may be adding to the
problem.
J) A water lubricated propeller shaft
bearing is worn prematurely after
few running hours.
Marine growth on the shaft.
Rotate shaft through two turns
every second day to break away
shaft deposits
26
APPLICATION DESIGN
5) APPLICATION DESIGN
a) Application Design
b) Interference
c) Bonding
d) Bore Closure
e) Running Clearance
f) Thermal Expansion Allowance
g) Absorption Allowance
h) Minimum Installed Clearance
i) Using the Thordon Bearing Sizing
Calculation Program
j) Step by Step Manual Calculations
k) Sample Manual Calculations
l) Keyed Tubular Bearing Calculations
m) High Pressure Bearings
n) Vertical Pump Bearings: Dry Start-up
a) APPLICATION DESIGN
The final dimensions of a Thordon bearing will depend on
how it is to be fitted. The selection of the best method
of fitting is extremely important and is dependent on
application requirements.
Thordon bearings are usually fitted either by installing
with interference or by bonding. In certain applications
mechanical keeper strips or keys are used to assist
interference fits. If a bearing is to be press fitted, then
interference and bore closure need to be considered in
the calculation along with running clearance, water swell
and thermal allowances. However, if it is to be bonded
into a housing, then only the latter three factors need
to be considered.
Thordon Bearings Inc. has developed a computer
program for calculating the dimensions of Thordon
bearings. This program greatly simplifies the
dimensioning process. Using the Thordon Bearing
Sizing Calculation Program is the preferred method
of calculating dimensions for Thordon bearings.
The explanations below are provided mainly to facilitate
understanding of the calculation parameters. Sample
manual calculations are provided for reference.
The following parameters should be considered:
Housing Size and Tolerance
Shaft Diameter and Tolerance
Length of Bearing
Operating Temperatures
Machine Shop Temperature
Type of Lubrication
Retention Method
b) INTERFERENCE
One of the basic and important differences between
Thordon and other bearing materials is that Thordon
requires more interference. This is due to the nature
of the material. The larger interference does not cause
any significant problems, but it must be taken into
consideration to ensure that Thordon bearings have
Thordon elastomeric bearings shrink on the O.D. and I.D.
as the temperature decreases. Due to the high coefficient
of thermal expansion (or contraction), compared to metal,
it is necessary to allow for this factor when the operating
environment drops below ambient. For calculation
purposes, we assume ambient (machine shop) temperature
to be 21&deg;C (70&deg;F). The Thordon Bearing Sizing Program
calculates dimensions at 21&deg;C (70&deg;F) ambient temperature
and then provides adjustments to the dimensions to suit
actual ambient temperature in the machine shop at time
of machining.
In the Housing Interference graphs (Figures 20 and 21),
the required cold temperature interference has been
calculated for XL &amp; SXL increments of 10&deg;C for metric
sizes and 20&deg;F for imperial sizes, below machine shop
ambient temperatures.
Thordon bearings installed with an interference fit can
be done with either a press fit or a freeze fit. An entry
chamfer on the bearing and/or a rounded corner on the
housing will facilitate press fitting. The press in force per
mm (inch) of bearing can be calculated as follows:
F(kg) = interference (mm) x wall thickness (mm) x length(mm) x 22
housing bore (mm)
F(N) = interference (mm) x wall thickness (mm) x length(mm) x 220
housing bore (mm)
F(lbs.) = interference (”) x wall thickness (”) x length(“) x 32000
housing bore (”)
When freeze fitting a Thordon bearing, the selection
of a suitable cooling agent depends on the temperature
differential for which the bearing’s interference fit is
designed. [Temperature differential is the difference
between ambient machine shop temperature and the
coldest temperature to which the installed bearing will
be exposed during operation.] If the differential is 40&deg;C
(100&deg;F) or less, then Dry Ice can normally be used. If
the differential is greater than 40&deg;C (100&deg;F), the use
of Liquid Nitrogen is recommended. The amount of
shrinkage that can be expected can be estimated using
the following information:
Each 10&deg;C decrease in temperature will result in an
approximate decrease in diameter of 0.0014mm/mm
of diameter.
27
Figure 20a: Housing Interference: XL Bearings (Metric)
recommended for Thordon HPSXL.
This material should be bonded
in place.
28
HOUSING BORE (inches)
On the removal of an
interference fit bearing from
the housing, it will recover a
portion of its total deflection
almost immediately, and then
it will slowly recover the
balance of the interference
except for the compression
set portion. In tests,
recovery based on standard
interference is over 90%
of initial deflection over a
period of several weeks.
NOTE: Interference fit is not
HOUSING BORE (mm)
Each 10&deg;F decrease in
temperature will result
in an approximate decrease
in diameter of 0.0008
inches/inch of diameter.
Figure 20b: Housing Interference: XL Bearings (Imperial)
APPLICATION DESIGN
Figure 21b: Housing Interference: SXL Bearings (Imperial)
HOUSING BORE (inches)
Figure 21a: Housing Interference: SXL Bearings (Metric)
HOUSING BORE (mm)
APPLICATION DESIGN
29
APPLICATION DESIGN
Both can influence axial compression. It also depends
on the coefficient of friction of the bearing material.
c) BONDING
As indicated in Section 4(i)-iii, bonding is an alternative
to interference fitting. Interference fit is not normally
used when bearings are bonded in place. The O.D. of the
bearing should be the housing diameter less an allowance
for the thickness of the bonding agent. The Thordon
Bearing Sizing Calculation program provides detailed
the calculation example in Section 5 (j)-2.
Thordon Bearings Inc. has extensively studied two bore
closure theories. Theory A does not allow for axial
movement in the calculations and Theory B does allow
for axial movement. Figure 22 shows typical test results.
For dimensioning Thordon bearings, Theory A has been
selected as the safest way of estimating bore closure
because it offers a greater running clearance.
To ensure good results are achieved, the procedures
for bonding using Thordon approved adhesives must
be followed, as outlined in Appendix 1.
The field results have been mixed, with most being close
to Theory A. Figures 23 and 24 reflect Theory A with
a maximum bore closure factor of 1.45 for Thordon XL
and Composite and 1.25 for Thordon SXL and COMPAC.
If required, actual testing in a given application can
develop more precise figures. The Thordon Bearing Sizing
Calculation program also uses Theory A for calculating
bore closure.
d) BORE CLOSURE
When a Thordon bearing is installed with an interference
fit, the inside diameter reduces due to volumetric
displacement. The actual bore closure value varies
depending on the surface finish on the outside diameter
of the bearing and the inside diameter of the housing.
Bore closure is expressed as a factor which is applied to
the average interference. It is added to the bearing I.D.
Figure 22: Thordon BoreTHORDON
Closure TestBORE
ResultsCLOSURE TEST RESULTS
OUTSIDE DIAMETER (mm)
0
50
100
150
200
250
300
350
400
450
500
550
600
650
1.7
1.6
BORE CLOSURE LIMITS
for 12.7mm (1/2&quot;) WALL
1.5
BORE CLOSURE FACTOR
XL
1.4
1.3
SXL
CONTRACTS DIAMETRICALLY ONLY : NO AXIAL GROWTH
1.2
THEORY &quot;A&quot;
1.1
1.0
CONTRACTS DIAMETRICALLY : WITH AXIAL GROWTH
THEORY &quot;B&quot;
0.9
0
0
0
0
0
10
12
14
OUTSIDE DIAMETER (inches)
FIG. 19
30
16
18
20
22
24
26
APPLICATION DESIGN
BORE CLOSURE FACTOR
FOR VARIOUS WALL THICKNESSES
METRIC
%BORE
BORE
CLOSURE
CLOSURE
FACTOR
Figure 23: Bore Closure Factor For Various Wall Thicknesses, Metric
2.0
200
1.8
180
WALL THICKNESS (mm)
160
1.6
50
XL and Composite
40
1.4
140
30
SXL and COMPAC
15
20
10
1.2
120
5
3
1.0
0
25
50
75
100
150
200
250
300
350
400
450
500
550
100
600
HOUSING
I.D. (mm)
HOUSING
I.D. (mm)
NOTE: This graph has been limited for use up to
maximum
1.25
bore closure
for SXL, of
and
a for
Note: This graph has been limited for use up to a maximum bore closure factor ofa1.25
for SXLofand
COMPAC,
and a maximum
1.45
maximum of 1.45 bore closure for XL.
XL and Composite.
PERCENTAGE BORE FACTOR
FOR VARIOUS WALL THICKNESSES
FIG. 20
IMPERIAL
BORE
CLOSURE FACTOR
BORE
CLOSURE
FACTOR
Figure 24: Bore Closure Factor For Various Wall Thicknesses, Imperial
WALL THICKNESS (inch)
XL and Composite
SXL and COMPAC
HOUSING I.D. (inches)
HOUSING I.D. (inches)
Note: This graph has been limited for use up to a maximum bore closure factor of 1.25 for SXL and COMPAC, and a maximum of 1.45 for
XL and Composite.
e) RUNNING CLEARANCE
NOTE: This graph has been limited for use up to a
maximum of 1.25 bore closure for SXL, and a
frictional heating of the bearing during
maximum of 1.45 bore closure for XL.
Recommended running clearances for Thordon bearings,
as well as all other non-metallic materials, are usually
more generous than those specified for metallic bearings.
Running clearance is necessary for the establishment of a
satisfactory liquid lubricant film. It also includes a margin
of safety to allow for bore reduction as a result of
operation. Figures
25 and 26 illustrate the diametrical running clearance
requirements for industrial and marine applications.
FIG. 21
Diametrical running clearance is the total difference in
dimension between the final installed inside diameter
of the bearing after accounting for the effects of
temperature and water absorption, and the outside
diameter of the shaft.
31
APPLICATION DESIGN
MINIMUM RUNNING CLEARANCE FOR THORDON BEARINGS
RELATED TO SHAFT DIAMETER
METRIC
MINIMUM RUNNING CLEARANCE (mm)
Figure 25: Minimum Running Clearance For Thordon Bearings
Related To Shaft Diameter, Metric
2.40
2.40
2.20
2.20
2.00
2.00
1.80
1.80
N
TATIO
L RO
FUL
N
TATIO
L RO
FUL
1.60
1.40
1.60
1.40
1.20
1.20
INE
MAR
1.00
1.00
IAL
STR
INDU
.80
.60
IAL
STR
INDU
AND
E
IN
MAR
.40
.20
.80
N
ROTATIO
LIMITED
.60
L
USTRIA
AND IND
MARINE
.40
.20
.00
.00
0
25
50
75 100
150
200
250
300
350
400
450
500
550
600
650
700
750
SHAFT OR (SLEEVE) DIA. (mm)
Note: Small bearing clearances reflect industrial standards. Larger marine bearings, 150mm and above are given greater clearance to reflect
NOTE: Where applicable, additional allowance must
NOTE: Small bearing clearances reflect industrial
ClassLarger
Societymarine
requirements.
standards.
bearings, 150mm and above
be made for thermal expansion and water swell. Refer
Note:
Where
applicable,
allowances
must be made for thermal expansion and water swell.
Steps
5/6 in Calculation
Procedures.
are
given
greater
clearance
to reflect
Class Society
to Refer
Stepsto5/6
in Calculation
Procedures.
requirements.
Figure 26:
FIG. 22
MINIMUM RUNNING CLEARANCE FOR THORDON BEARINGS
Minimum Running Clearance
For Thordon
RELATED
TO SHAFT Bearings
DIAMETER
IMPERIAL
Related To Shaft Diameter, Imperial
SHAFT OR (SLEEVE) DIA. (inches)
Smallclearances
bearing clearances
reflect industrial
NOTE:
NOTE:
Note: Small
bearing
reflect industrial
standards. Larger marine bearings, 6&quot; and above are
given When
greaterapplicable,
to reflect allowance must
standards. Larger marine bearings, 6” and above are
be made for thermal expansion and water swell. Refer
Class
Society
requirements.
given greater clearance to reflect Class Society
to Steps 5/6 in Calculation Procedures.
Note: Where
applicable, additional allowances must be made for thermal expansion and water swell. Refer to Steps 5/6 in Calculation Procedures.
requirements.
32
APPLICATION DESIGN
In oscillating motion applications, where heat build up
is not as likely to occur, running clearances can be
reduced as shown in Figures 25 and 26.
Inadequate running clearances result in bearing failure
characterized by a “smeared” or “wiped” bearing I.D.
from the bearing length to allow room for the axial
expansion before encountering the retainers. The axial
thermal expansion allowance is calculated using the
following formula.
Ct (axial) = L α (To - Ta)
NOTE 1: If sufficient axial thermal expansion clearance is not provided,
the bearing will still expand. It will either dislodge the bearing retainers
or, instead of expanding axially, it will expand more diametrically, reducing
the running clearance of the bearing. This can result in bearing failure.
NOTE 2: Thermal expansion allowances calculated using the Thordon
Bearing Sizing Program might be slightly different from those done
manually. This is because the Sizing Program uses a more complex
formula to calculate the absorption allowance. The computer program
calculated allowance is more accurate than the manual calculations.
g) ABSORPTION ALLOWANCE
Typical example of a wiped bearing.
NOTE 1: In certain bearing configurations, where there is no
unidirectional load such as vertical pumps and vertical hydro turbines,
reduced running clearances are possible. In these configurations,
bearings can be designed with running clearances of 0.075% to 0.1%
of shaft diameter. Bearing designs with tighter running clearances are
NOTE 2: For some specific applications such as Thor-Lube stern tube
bearings, special running clearances are required. Please consult
Thordon Bearings for details.
f) THERMAL EXPANSION ALLOWANCE
Thermal Expansion Allowance (Ct) is an additional
clearance that must be taken into account when the
bearing will operate at temperatures above ambient
(machine shop) temperature. The diametrical Ct is
calculated based on the coefficient of thermal expansion
of Thordon using the following formula.
Ct (diametrical) = 2 W.T. α (To - Ta)
Thordon normally absorbs liquid at a rate of 1.3% by
volume, although in warmer liquids the expansion by
volume can reach a rate of 2%. Although considerably
less than most competitive non-metallic products, this
expansion must be taken into account because it results
in bore reduction as well as a slight increase in
interference fit.
The diametrical (bore closure) effect of the Absorption
Allowance (Cs) is calculated using the following formula.
Cs (diametrical) = W.A.F. x W.T.
where W.A.F. is the Water Absorption Factor determined
from Figure 27 for the approximate maximum operating
temperature. W.T. is wall thickness.
For example: if the highest operating temperature is 21&deg;C
(70&deg;F), the W.A.F. is 0.011. This clearance is then added
to the minimum running clearance obtained from Figure
25 or 26.
In applications where the bearing is being operated in a
liquid and axially retained, an axial absorption allowance
must be deducted from the machined bearing length to
Figure 27: Water Absorption Factor (W.A.F.)
For Various Water Temperatures
WATER ABSORPTION FACTOR (W.A.F.) FOR VARIOUS WATER TEMPERATURES
For a temperature range of 0&deg;C to 30&deg;C (32&deg;F to 86&deg;F)
XL and Composite: α = 0.000148/&deg;C (0.000082/&deg;F)
SXL and COMPAC: α = 0.000151/&deg;C (0.000084/&deg;F)
NOTE: A Directory of symbols used is found on the inside front cover.
This clearance (Ct) is then added to the minimum running
clearance as determined from Figure 25 or 26.
In applications where the bearing is being axially retained
and is operating at temperatures above ambient, an
axial thermal expansion allowance must be deducted
WATER ABSORPTION FACTOR (W.A.F.)
α = Coefficient of Thermal Expansion for Thordon
as follows:
XL, SXL, COMPAC
and Composite
MAXIMUM OPERATING TEMP.
IN WATER
TEMPERATURE &deg;C (&deg;F)
33
APPLICATION DESIGN
allow room for the axial expansion before encountering
the retainers. The axial absorption allowance for an
interference fit bearing is calculated using the following
formula.
Cs (axial) = .005 x Length of Bearing
NOTE: If sufficient axial absorption clearance is not provided, the
bearing will still expand, dislodging the bearing retainers or, instead
of expanding axially, it will expand more diametrically reducing the
running clearance of the bearing. This can result in bearing failure.
h) MINIMUM INSTALLED CLEARANCE
As indicated in the following examples, the ID of
a bearing is calculated by adding the bore closure
(if applicable), running clearance, thermal expansion
allowance and absorption allowance to the maximum
shaft diameter. When the bearing is fitted into the
housing, the bore closure (if applicable) happens, so
the allowance is not a factor. What is left is running
clearance, thermal expansion allowance and absorption
allowance. The sum of these three factors is what is called
“Minimum Installed Clearance”. This is clearly indicated
in the Thordon Bearing Sizing Calculations. When the
bearing is operating, the thermal expansion allowance
will disappear when the maximum operating temperature
is reached, and the absorption allowance will disappear
as the bearing gradually absorbs the lubricating liquid.
Running clearance will be the only clearance left.
Minimum Installed Clearance is used as an important final
check before putting the bearing into service. If the
measured clearance after fitting is less than the Minimum
Installed Clearance, then there is a high probability that
the bearing will fail. The problem should be fixed before
the bearing enters service.
i) USING THE THORDON BEARING
SIZING CALCULATION PROGRAM
A computer program is available to calculate the sizing of
Thordon bearings. It takes into account all of the factors
covered in the application design section of this manual
and greatly simplifies the calculation process. The program
is available from your Thordon distributor or Thordon
Bearings Inc.
The Thordon Bearing Sizing Calculation Program is only
as reliable as the information entered. As with manual
dimension calculations, the same care must be taken to
ensure that all inputs are correct. The current program
is the result of more than 15 years of work with
computer-based Thordon dimension calculations.
The Bearing Sizing Calculation Program will go beyond
the manual calculations in some cases. For example, it
34
will add interference if required to ensure that relatively
thin walled bearings have sufficient interference. It
will also indicate when a bearing wall is too thin for
interference fit. A bond fit will be recommended. The
program will also review tolerances and reject applications
where the housing tolerance is more than 1/3 of the
running clearance.
Detailed help screens are available throughout the
program if you have questions regarding a specific topic.
NOTE: The values calculated from the Bearing Sizing Calculation Program
may be slightly different than those calculated manually using this
manual due to differences resulting from inaccuracies in reading values
from the graphs etc. In general the computer program is more accurate
than the manual calculation process.
The following are examples of the Sizing Program used
to calculate typical bearing dimensions:
1) SAMPLES USING BEARING SIZING
CALCULATION PROGRAM
a) METRIC EXAMPLE
FIT: Interference
Given Data
1. Type of Operation
2. Shaft Diameter
3. Bearing Housing
4. Housing Length
5. Operating Temp.
6. Ambient Temp.
7. Environment
MATERIAL: XL
Marine Propeller Shaft
100mm +0.00/-0.13mm
150mm +0.08mm/-0.00 mm
400mm
Min. -2&deg;C Max. 45&deg;C
21&deg;C
Water
The Sizing Program gives the following results:
Machined Bearing Inside Diameter:
102.30mm +0.13, -0.00
Machined Bearing Outside Diameter:
151.00mm +0.13, -0.00
Minimum Installed Diametrical Clearance: 0.89mm
Machined Bearing Length: 396.26mm +0.00, -0.50
Bearing Wall Thickness: 24.35mm
b) IMPERIAL EXAMPLE
FIT: Interference
Given Data
1. Type of Operation
2. Shaft Diameter
3. Bearing Housing
4. Housing Length
5. Operating Temp.
6. Ambient Temp.
7. Environment
MATERIAL: XL
Marine Propeller Shaft
4” +0.000”/-0.005”
6” +0.003”/-0.000”
16&quot;
Min. 28&deg;F Max. 113&deg;F
70&deg;F
Water
APPLICATION DESIGN
The Bearing Sizing Program Gives the Following Results:
Machined Bearing Inside Diameter:
4.091” +0.005”/-0.000”
Machined Bearing Outside Diameter:
6.040” +0.005”/-0.000”
Minimum Installed Diametrical Clearance: 0.035”
Machined Bearing Length: 15.855” +0.000”/-0.010”
Bearing Wall Thickness: 0.974”
The Thordon Bearing Sizing program can also be used
to do the calculations below quickly and accurately.
The program will provide machining dimensions for the
bearing O.D., for either interference or bond fit. For
the machined bearing I.D., run the appropriate calculation
for an interference or bonded fit, and then add the
“Minimum Installed Clearance” to the shaft diameter
to obtain the required bearing I.D. for machining.
2) SAMPLE CALCULATION WORKING WITH THE
THORDON BEARING SIZING CALCULATION PROGRAM
a) METRIC EXAMPLE: Bearing machined after
fitting into housing
FIT: Interference Fit, machined after fitting in housing
MATERIAL: SXL
Given Data
1. Type of Operation
Ind./Vertical Turbine Pump
2. Shaft Diameter
100mm +0.00mm/-0.13mm
3. Bearing Housing
150mm + 0.04mm/-0.00mm
4. Housing Length
200mm
5. Operating Temp.
Min. 10&deg;C Max. 30&deg;C
21&deg;C
6. Ambient Temp.
7. Environment
Water
Use the Thordon Bearing Sizing Calculation Program
to calculate the finished dimensions of the bearing.
In this case the program gives the following results:
Machined Bearing I.D.: 101.55mm +0.13mm/-0.00mm
Machined Bearing O.D.: 150.77mm +0.13mm/-0.00mm
Minimum Installed Diametrical Clearance: 0.53mm
Machined Bearing Length: 198.66mm +0.00mm/-0.50mm
Step 1: Bearing O.D. is machined to 101.55mm as per
Sizing Calculation program
Step 2: Fit bearing into housing
Step 3: Machine bearing I.D. to maximum shaft diameter
plus minimum installed clearance = 100+ 0.53 =
100.53mm. (The Thordon Bearing Sizing Calculation
Program will calculate minimum installed
clearance. The difference between the value in
Step 3 and machined bearing is bore closure.)
NOTE: When final machining of the bearing bore is done after it is
installed in the housing, care must be taken because this method
removes stressed material that is developing the “grip” of the bearing
within its housing. Only minimum material must be removed. For
ungrooved bearings, this machining stage must not remove more than
5% of the wall thickness.
For grooved bearings, it is not as important because the bore material
is much less stressed, however machining should be limited to 10%
of the wall thickness or 25% of the groove depth, whichever is less.
Lubrication grooves must always be machined prior to fitting
the bearing into the housing.
b) IMPERIAL EXAMPLE: Bearing machined after
fitting into housing
FIT: Interference Fit, machined after fitting in housing
MATERIAL: SXL
Given Data
1. Type of Operation
Ind./Vertical Turbine Pump
2. Shaft Diameter
4” +0.000/-0.005”
3. Bearing Housing
6” + 0.003”/-0.000
4. Housing Length
8”
5. Operating Temp.
Min. 50&deg;F Max. 86&deg;F
6. Ambient Temp.
70&deg;F
7. Environment
Water
Use the Thordon Bearing Sizing Calculation Program
to calculate the finished dimensions of the bearing.
In this case the program gives the following results:
Machined Bearing I.D.: 4.062” +0.005”/-0.000”
Machined Bearing O.D.: 6.032” +0.005”/-0.000”
Minimum Installed Diametrical Clearance: 0.021”
Machined Bearing Length: 7.945” +0.000”/-0.020”
Step 1: Bearing O.D. is machined to 6.032” as per
Thordon Bearing Sizing Calculation Program.
Step 2: Fit bearing into housing.
Step 3: Machine bearing I.D. to maximum shaft diameter
plus minimum installed clearance = 4 + .021 =
4.021”. (The Thordon Bearing Sizing Calculation
Program will calculate minimum installed
clearance. The difference between the value in
Step 3 and machined bearing is bore closure.)
NOTE: When final machining of the bearing bore is done after it is
installed in the housing, care must be taken because this method
removes stressed material that is developing the “grip” of the bearing
within its housing. Only minimum material must be removed.
For ungrooved bearings, this machining stage must not remove more
than 5% of the wall thickness.
For grooved bearings, it is not as important because the bore material is
much less stressed, however machining should be limited to 10% of the
wall thickness or 25% of the groove depth, whichever is less.
Lubrication grooves must always be machined before the bearing is
fitted into the housing.
35
APPLICATION DESIGN
j) STEP BY STEP MANUAL CALCULATIONS
1) Interference Fit
For a bearing being fitted into a housing using an
interference fit, the following steps need to be taken
to ensure correct sizing.
Bearing O.D.
Step 1: The interference is determined from Figures 20(a)
and (b) or 21(a) and (b) and added to the
maximum housing diameter to give the minimum
machined bearing O.D. Allowances for operating
temperatures below ambient machine shop
conditions are determined directly off Figures
20(a) and (b) or 21(a) and (b) using the
appropriate curve for the number of degrees
below ambient.
Bearing I.D.
Step 2: The bore closure factor, determined from Figures
23 or 24, is multiplied by the average interference
(minimum interference plus 50% of housing
tolerance and 50% of machining tolerance on
bearing O.D.) to give the bore closure allowance.
Step 3: The running clearance is determined from
Figures 25 or 26.
Step 4: If the bearing is subjected to temperatures
higher than machine shop ambient, the thermal
Step 5: The water absorption factor is determined from
Figure 27 and multiplied by the wall thickness
(if applicable).
Step 6: The machined I.D. is determined by adding bore
closure allowance, running clearance, temperature
allowance (if applicable) and absorption allowance
(if applicable) to the maximum shaft diameter.
2) Bonded Fit
For an application requiring the Thordon bearing to be
bonded into the housing, the following steps are required.
Step 1: The O.D. of the bearing should have a 0.25mm
(.010”) to 0.50mm (.020”) clearance to the
housing, to provide for an adhesive film.
Step 2: Running clearance is determined from
Figures 25 or 26.
Step 3: Thermal expansion allowance is calculated
if necessary.
Step 4: Water absorption factor is determined from
Figure 27 and is multiplied by the wall thickness
(if applicable).
36
Step 5: The I.D. of the bearing is determined by adding
the running clearance, thermal allowance
(if applicable) and water absorption allowance
(if applicable) to the maximum shaft diameter.
3) Machining I.D. after fitting into housing or
“dummy” housing
As indicated in the design guide, it is occasionally
preferable to machine the final cut on the I.D. of a
Thordon bearing after it has been fitted into its housing,
or into a “dummy” housing.
The dimension calculations are the same whether the
housing is final or “dummy”.
Step 1: Machine the O.D. of the bearing to
the dimensions calculated in Step 1 of
section j) 1 or 2.
Step 2: Fit the bearing into the housing or “dummy”
housing using a freeze, press or bond fit
as appropriate.
Step 3: Running clearance is determined from
Figures 25 or 26.
Step 4: Thermal expansion allowance is calculated
if necessary.
Step 5: Water absorption factor is determined from
Figure 27 and is multiplied by the wall
thickness (if applicable).
Step 6: The I.D. of the bearing is determined by adding
the running clearance, thermal allowance
(if applicable) and water absorption allowance
(if applicable) to the maximum shaft diameter.
(Because the bearing is already fitting into the
housing, bore closure is no longer a factor.)
Step 7: If freezing has been used, allow time for the
before machining.
NOTES:
When final machining of the bearing bore is done after it is installed in
the housing, care must be taken because this method removes stressed
material that is developing the “grip” of the bearing within its housing.
Only minimum material must be removed.
For ungrooved bearings, this machining stage must not remove more
than 5% of the wall thickness.
For grooved bearings, it is not as important because the bore material
is much less stressed, however machining should be limited to 10%
of the wall thickness or 25% of the groove depth, whichever is less.
Lubrication grooves must always be machined before the bearing
is fitted into the housing.
APPLICATION DESIGN
k) SAMPLE MANUAL CALCULATIONS
(a) METRIC
FIT: Interference
MATERIAL: SXL
Given Data
1. Type of Operation
2. Shaft Diameter
3. Bearing Housing
4. Housing Length
5. Operating Temp.
6. Ambient Temp.
7. Environment
Marine Propeller Shaft
250mm + 0.00 / -0.10mm
300mm +0.10/-0.00mm,
1000mm
Min. -2&deg;C Max. 30&deg;C
21&deg;C
Water
Outside Diameter
Step 1
Interference for a 300mm diameter housing operating
at 23&deg;C below ambient from Figure 20(a).
= 1.85mm
Step 1-1
Bearing O.D. = Maximum Housing + Interference
= 300.10 + 1.85
= 301.95mm
With standard machining tolerance
Bearing O.D. = 301.95 + 0.13/-0.00mm
Inside Diameter
Step 2
Bore closure factor from Figure 23 = 1.147
Actual bore closure = average interference x
bore closure factor
Avg. interference = Interference (Step 1) + 50% of
Housing and Bearing O.D. tolerance.
= 1.85 + (.10 + .13) = 1.97mm
2
Actual bore closure is 1.97 x 1.147
= 2.26mm
Step 3
Basic running clearance for 250mm shaft
from Figure 25
= 0.96mm
Step 4
Thermal Expansion (Ct) = 2W α (To - Ta)
Ct = 2 x 25 x .000151 x 9
= 0.07mm
Step 5
Absorption Cs = W.A.F (from Figure 27) x wall thickness
= 0.0124 x wall thickness
Cs = 0.0124 x 25
Total Allowance = Steps 2 + 3 + 4 + 5
= 0.31mm
= 3.60mm
Step 6
Bearing I.D. = maximum shaft diameter +
total I.D. allowance
= 250.00 + 3.60mm
= 253.60mm
with standard machining tolerance
Bearing I.D. = 253.60 +0.13/-0.00mm
Minimum Installed Clearance
(for final check) = steps 3 + 4 + 5
= 1.34mm
Bearing Length
Step 1
Axial thermal expansion
Ct = 1000 x .000151 x 9
= 1.36mm
Step 2
Axial absorption allowance Cs = .005 x 1000 = 5.00mm
Step 3
Machined bearing length = housing length – axial
thermal expansion allowance – axial absorption
allowance = 1000-1.36-5.00 = 993.64mm
With standard machining tolerance length
= 993.64 +0.00/-1.00mm
NOTES:
a) Calculations involving bearings in limited rotation applications are
the same as above, except for a decrease in running clearance required
in Step 3 as shown in Figure 25 or 26.
b) If the bearing is not immersed in a liquid, the allowance for water
absorption calculated in step 5 is not required.
c) To minimize tolerance build up in the installed running clearance
of a press fit bearing, the bearing can, if feasible, be machined after
installation in the housing. See section (i)3 above for details.
(b) IMPERIAL
FIT: Interference
Given Data
1. Type of Operation
2. Shaft Diameter
3. Bearing Housing
4. Housing Length
5. Operating Temp.
6. Ambient Temp.
7. Environment
MATERIAL: SXL
Marine Propeller Shaft
10” +0.000”/-0.005”
12” +0.005”/-0.000”
40”
Min. 28&deg;F Max. 86&deg;F
70&deg;F
Water
Outside Diameter
Step 1
Interference for a 12” housing diameter bearing operating
at 42&deg;F below ambient from Figure 21(b).
= 0.074”
Step 1-1
Bearing O.D.
= Maximum Housing + Interference
= 12.005” + 0.074”
= 12.079”
With standard machining tolerance
Bearing O.D. = 12.079” + 0.005”/-0.000
37
APPLICATION DESIGN
Inside Diameter
Step 2
Bore closure factor from Figure 24 = 1.148
l) KEYED TUBULAR BEARING
CALCULATIONS
Actual bore closure = average interference x
bore closure factor
Avg. interference = Interference (Step 1) + 50% of
Housing and Bearing O.D. tolerance
= .074 + (.005 + .005) = .079”
2
Actual bore closure is 0.079” x 1.148
= 0.091”
Step 3
Basic running clearance for 10” shaft from
Figure 26
= 0.038”
Step 4
Thermal Expansion (Ct) = 2W α (To - Ta)
Ct = 2 x 1 x .000084 x 16
= 0.003”
Step 5
Absorption Cs = W.A.F. (from Figure 27) x wall thickness
= 0.0124 x wall thickness
Cs = 0.0124 x 1”
= 0.012”
Total Allowance = Steps 2 + 3 + 4 + 5
Thordon bearings are often installed with both an
interference fit and one or two sets of locking keys.
To size the Thordon bearings and split gap widths to
obtain the correct interference for a keyed bearing
application, the following procedure should be used.
1. Calculate the bearing dimensions based on a normal
tube and an interference fit. The calculations can
be done using the Thordon Bearing Sizing Calculation
Program or in the step-by-step manner detailed in
section 5(j) of this manual.
2. Machine the bearing according to the calculated
dimensions.
3. Measure the circumferential width of the key(s) and
measure or approximate the width of the cut on the
side opposite the key in the case of a single key.
See Figure 28.
= 0.144”
Figure 28: Measuring Key Widths
Step 6
Bearing I.D. = maximum shaft diameter +
total I.D. allowance
= 10” + 0.144”
= 10.144”
with standard machining tolerance
Bearing I.D. = 10.144” +0.005”/-0.000
Minimum Installed Clearance
(for checking) = steps 3 + 4 + 5
= 0.053”
Bearing Length
Step 1
Axial thermal expansion
Ct = 40 x .000084 x 16
=0.054”
Step 2
Axial absorption allowance Cs = .005 x 40
=0.200”
Step 3
Machined Bearing Length = housing length – axial
thermal expansion allowance – axial absorption allowance
= 40-0.054-0.200 = 39.746”
With standard machining tolerance bearing length
= 39.746” +0.000/-0.040”
NOTES:
a) Calculations involving bearings in limited rotation applications are
the same as above, except for a decrease in running clearance required
in Step 3 as shown in Figure 25 or 26.
b) If the bearing is not immersed in a liquid, the allowance for water
absorption calculated in step 5 is not required.
c) To minimize tolerance build up in the installed running clearance
of a press fit bearing, the bearing can, if feasible, be machined after
installation in the housing. See section (i)3 above for details.
38
4. Cut the slot(s) in the bearing so the total width of
material removed equals the width of the keys / keyset.
Ensure that the combined circumferential interference
of bearing and key(s) is the same as for a non-split
bearing.
5. If more than one key or keyset is fitted, then the
bearing is slotted accordingly, the slots logically
positioned to suit the keys and the material
removed in each slot equal to the width of the
corresponding keys.
Note: The same approach should be taken when working with a split
bearing that will be interference fitted with no keys. It is important
to maintain the circumference after splitting. The easiest approach
is to fully machine the bearing as a tube and then split it. Use the
Thordon Bearing Sizing Calculation Program to calculate the bearing
dimensions as if it were not split. Then add to the O.D. and I.D. the
circumferential effect of the thickness of the splitting cuts – total
thickness of cuts/π.
APPLICATION DESIGN
m) HIGH PRESSURE BEARINGS
Thordon has two grades for high pressure bearing
applications. The first is ThorPlas&reg;, a new homogeneous
non elastomeric material. Details on ThorPlas&reg; are
provided in a separate manual. The other grade for
high pressure bearing applications is Thordon HPSXL
TRAXL, which is specified in many industrial and marine
applications. HPSXL TRAXL bearings are ideally suited to
applications where the loads are high and conventional
lubrication is not used.
The cold bonding process is used when the application
requires a combination of relatively high pressure
capability and thicker (greater than 1.5mm or 0.060”)
wall. The pressure rating decreases, however, as the wall
thickness increases, due to the decreasing shape factor.
Much tighter running clearances can be achieved with
HPSXL TRAXL bearings compared to Thordon sleeve
bearings. There are a number of factors that contribute
to this:
All machining is performed after the Thordon material
is bonded into the bearing shell. Therefore, tolerance
build up is minimized.
Typical applications include hydro-turbine wicket gates
and linkages, lock gate supports, stern rollers, cranes
and construction equipment pivot points.
Due to the rigid metal shell, and the support that
it provides to HPSXL, both the O.D. and I.D. can be
machined to tighter tolerances.
Thordon HPSXL TRAXL bearings are a composite design
consisting of a thin layer of Thordon HPSXL bonded in
a metallic shell.
As outlined in the section covering Selection Process
on page 23, it is possible to achieve operating pressures
up to 55.0 MPa (8000 psi) with permissible peak static
pressures up to 70.0 MPa (10,000 psi) or higher with
HPSXL TRAXL bearings.
These pressure ratings are achieved through the
combination of several factors.
The applications are either oscillating or very slow
speed operation so that frictional heat build up is
not a consideration.
The bearing is designed with a very high shape
factor (typically over 100). This means that
the wall thickness of the bearing is very thin
(usually 1.5mm (0.060”) or less).
Optimum high pressure results are obtained using Thordon
HPSXL TRAXL in which HPSXL is bonded directly into a
specially grooved metallic shell. This bearing with HPSXL
as the wear surface is then press fit into the bearing
housing. Lower pressure applications can be done by
cold bonding a thin wall Thordon tube into a shell.
The pressure range for each method is illustrated in
Figure 29.
Figure 29: Pressure Range for Different
Manufacturing Methods
Manufacturing
Method
TRAXL
Cold Bonded
Pressure
Normal Operation
Peak Static
MPa
psi
MPa
psi
27.5 - 55.0
13.7 - 20.6
4000 - 8000
2000 - 3000
70.0 10,000
27.5 4,000
Design running clearance is reduced because rotation
is limited (frictional heat build up is not a concern).
Similarly, due to the thin wall, the thermal expansion
and absorption allowances are not significant.
The following design parameters should be considered in
the design of a Thordon high pressure bearing application:
• Interference
• Bore Closure
• Running Clearance
• Housing and Shaft Dimensions
• Bearing Dimensioning and Tolerances
NOTE 1: Absorption Allowance and Thermal Allowance are normally
assumed to be insignificant because the Thordon wall thickness in a
HPSXL TRAXL bearing is usually 1.5mm (0.060”) or less. If the thickness
of HPSXL is greater than this, then the Absorption Allowance and
Thermal Expansion should be considered.
NOTE 2: The calculations for HPSXL TRAXL bearings are different from
those for full form Thordon bearings because the relatively thin HPSXL is
fitted into a metallic shell. Calculations such as interference and bore
closure are based on the properties of the metallic shell rather than on
the properties of the Thordon.
i)
Interference:
The amount of interference between the Thordon HPSXL
TRAXL bearing and the housing is dependent on the
operating conditions. As the pressure increases so must
the interference. The normal recommended interference
fit ranges from 0.025% to 0.100% of the O.D. depending
upon the size of the bearing. For larger bearings, the
percent interference is decreased.
Note: HPSXL TRAXL bearings should not be freeze fitted. There is a
significant risk that freezing, with dry ice or liquid nitrogen, could
damage the bond between the Thordon HPSXL and the metallic shell.
ii) Bore Closure:
NOTE: Thordon bearings can be designed to operate at higher pressures
information.
From practical experience the bore closure from an
interference fit between two metals is normally in the
39
APPLICATION DESIGN
range of from 75 to 95% of the interference. To ensure
that running clearance is adequate, an assumed bore
closure factor of 1 is recommended for calculation
purposes.
iii) Running Clearance:
The normal recommended running clearance is 0.1%
of shaft diameter with a minimum recommendation of
0.075mm (0.003”).
In applications where tighter tolerances are required
Bearings for guidance.
iv) Housing and Shaft Dimensions:
To obtain the optimum installed running clearance it is
necessary to control tightly the tolerances of not only the
bearing but also of the housing and the shaft. Excessive
housing bore or shaft tolerances translate directly into
additional running clearance requirements. If a project
involves a series of bearings as in a wicket gate assembly,
each position can be measured and numbered so that the
HPSXL TRAXL bearings can be specifically dimensioned for
each position.
v) Bearing Dimensioning and Tolerances:
The O.D. and I.D. of a Thordon HPSXL TRAXL bearing are
calculated as follows:
Bearing O.D. = Housing Diameter (maximum) + Normal
Interference
Bearing I.D. = Shaft Diameter (maximum) + Bore Closure
(maximum bearing O.D. - minimum housing
diameter) + Running Clearance
The standard machining tolerances of Thordon High
Pressure bearings are:
Bearing O.D.: +0.025mm/-0.000mm
(+0.001”/0.000”)
Bearing I.D.: +0.075mm/-0.000mm
(+0.003”/-0.000”)
n) VERTICAL PUMP BEARINGS:
DRY START-UP
Thordon SXL is widely used in vertical pumps because of
its ability to run dry on start-up. The length of time that
SXL can run dry in a vertical pump configuration usually
meets the requirements of the pump designer for dry
start-up. The Thordon Bearing Sizing Calculation Program
will automatically adjust the clearances when a dry
start-up vertical pump application is selected. For further
Thordon Bearings.
40
MACHINING
6) MACHINING &amp;
MEASURING
a) General Machining
b) Machining XL, SXL or COMPAC
c) Machining Composite
d) Dimensional and Surface Finish
Measurements
Virtually all operations that can be performed on metal,
including machining, drilling, tapping, shaping, routing,
sawing, milling and bonding, can be performed on
Thordon. Thordon can also be worked or shaped with
conventional hand tools, keeping in mind that carbide
tipped cutting blades should be used to prevent heat
build up when sawing.
b) MACHINING XL, SXL or COMPAC
i)
NOTE: Machining videos are available from Thordon Bearings or from
your local distributor. This is an excellent tool for understanding the
requirements for machining Thordon bearings.
a) GENERAL MACHINING
Cutting Tool
To machine Thordon it is critical that the correct
cutting tool be used. The tool must be designed to
slice the material and project it away from the
machined surface.
Thordon is a hard tough elastomeric polymer product
that can be easily machined. It is necessary, however,
to remember that Thordon is a non-metallic and must be
machined differently than metal. Due to the elastomeric
nature of Thordon it has a tendency to “move away” from
anything that exerts pressure on it, including machine
tools of all types. Thordon cannot be burnished or
chipped, it must be cut with a sharp tool. The importance
of sharp cutting tools cannot be overemphasized if
Thordon is to be successfully machined.
Some of the new cutting tools currently available provide
excellent results machining Thordon. They are extremely
sharp initially and hold their edge very well.
When thin wall bearings are being machined it is
important to recognize that the exertion of excess
pressure may actually deform the bearing. In some
situations it may be necessary to use modified chuck
jaws, to support the tube using a spider, plug or a
mandrel or to mount the tube using a faceplate.
Thordon Bearings recommends a tool bit manufactured
by Kennametal that is available worldwide. The tool
bit is Titanium Nitride PVD coated carbide and is
Kennametal part number: CPGT3251HP-KC730. The
tool holder is part number: SCMPN-083V.
When machining Thordon, a continuous streamer is
projected from the cutting tool. The cutting tool
must be sharp. After grinding, the conventional
cutting tool should be honed with an oilstone to
ensure a sharp cutting edge.
Cutting speeds are also important. Low feed rates
combined with too low a turning speed tend to produce a
rough cut due to the toughness and elastomeric nature of
Thordon. High speeds combined with a low feed rate may
produce excessive frictional heat, resulting in a gummy,
galled finish. The most suitable speed/feed combinations
are similar to those used when machining aluminum.
this manual, may seem excessive in comparison to metals.
Thordon, however, expands from temperature change and
submersion in liquids. Thordon also exhibits bore closure
shrinkage at a rate greater than 100% of interference.
This is due to the incompressible nature of Thordon. The
minimum installed clearance takes all of these factors
into account. As well, clearance for a liquid lubrication
film if the bearing is water or oil lubricated and safety
clearance for frictional heat build up are also accounted
for. The recommended running clearance should not be
decreased without first consulting your Thordon
distributor or Thordon Bearings Inc.
NOTE: If adequate running clearance is not provided, bearing failure is
almost certain.
Kennametal tool bit
41
MACHINING
There are a number of tool bits and holders offered in
the Kennametal KC730 series. The applicable ISO standards
are M05 - M20, S15 - S25. If you have trouble locating
It is important when machining Thordon and
particularly when boring, to ensure that the machining
streamer is removed from the work. If this is not done,
it will interfere with the cutting tool and a rough finish
will result.
NOTE: Due to the very elastic nature of the material, caution should
be taken when removing cuttings from the work area.
Bearing Diameter
Metric Imperial RPM Coarse Feed
75mm
150mm
300mm
450mm
600mm
750mm
900mm
3”
6”
12”
18”
24”
30”
36”
600
450
300
150
120
95
80
0.6mm/rev.
(0.025”/rev)
for HSS tool
Fine Feed
0.4mm/rev.
(0.015”/rev.)
for HSS tool
0.3mm/rev.
0.2mm/rev.
(0.012”/rev.) (0.007”/rev.)
for tipped tool for tipped tool
iii) Bearing Set Up
Machining - Partial length from a tube:
tool configuration when using conventional tool bits.
High speed steel can be used for SXL and COMPAC;
tungsten carbide tool bits are used with XL.
1) General Machining Tool Bit
General Machining Tool Bit
10
500&quot; SQ. HIGH SPEED STEEL
12.7 mm.
1/16&quot; R
1.5 mm.
3/16&quot; R
5 mm.
30˚
60˚
60˚
2) Step
Tool
Step Machining
Machining Tool
BitBit
SQUARE
A bearing that is being made from the partial length
of a tube can be chucked at one end in a normal 3 jaw
chuck, the O.D. rough machined, the I.D. finish machined,
the O.D. finish machined and then parted to length.
Care must be taken not to over tighten the chuck and
distort the tube.
Machining - I.D. - thin wall tube with soft jaw chuck:
3/16&quot; R.
5 mm.
30˚
10˚
1/16&quot; R.
30˚
1.5 mm.
ii) Machining Speeds and Feeds
Suggested turning speeds for bearings of various
diameters are provided in the chart in the next column.
NOTE 1: The turning and feed speeds are provided as a guide only.
The optimum speed may vary higher or lower depending on such
variables as the length of tube, the wall thickness, and how the bearing
is being supported, i.e. simply chucked, spider at chuck or on a full
length mandrel. As is common with all machining operations, some
experimentation is required to obtain optimum results.
NOTE 2: Cutting lubricants are not required and are not recommended.
42
To machine the I.D. of a thin wall tube, the O.D. should
be rough machined, the tube gripped in an extended soft
jaw chuck and the I.D. finish machined. The extended
chuck will grip and support the tube without deforming.
MACHINING
Machining - I.D. - thin wall tube with external sleeve:
A thin wall tube I.D. can also be machined by first
machining the O.D. to size, lightly pressing the tube into
a machined metal housing, chucking the housing and then
machining the I.D. of the tube. It is possible to obtain
tighter tolerances than those obtained with external soft
jaws with this method but it is more involved and usually
not necessary.
Machining - O.D. - full length of a lubrication grooved
bearing - supported on centres:
Machining - O.D. - machined steel plug or
After the I.D. of a tube has been finish machined, a
machined steel plug can be slip fit into the I.D. of the
bearing. On larger tubes a 3 or 4 arm spider can be set
to the inside diameter of the tube and located opposite
the chuck jaws. Both of these devices eliminate distortion
from chuck jaw pressure. A simply constructed 4-arm
spider is illustrated below. With either of these methods
it is necessary to add a 50mm (2”) chucking allowance
to the required length of the bearing.
Spider
SPIDER
Bar or Tube
SCREW &amp; LOCKNUT
After the I.D. of a bearing with lubrication grooves has
been finish machined the bearing can be chucked on
centres, driven by a key in one of the grooves and the
O.D. finish machined. This method is acceptable for
propeller shaft bearings, but will not yield the tight
tolerances required for pump bearings.
43
MACHINING
Machining - O.D.
Preferred Machining Method- O.D. and I.D. :
Bearings larger than 380mm (15”) O.D. are most easily
mounted for machining by lag screwing them to a
faceplate. The faceplate can then be set up on a vertical
mill, or chucked in the lathe. An additional 50mm (2”)
must be added to the required length of the bearing as
a chucking allowance. The faceplate is centered as
accurately as possible and then screwed to the tube using
lag screws into pre-drilled holes. After mounting, the tube
can be trued for machining, if required, by loosening the
screws and adjusting the position of the tube using the
slots in the faceplate.
The O.D. of the tube is rough machined first, then the I.D.
finish machined, the O.D. finish machined and then the
bearing is parted to length from the tube. If the bearing
is too large to safely catch as it is parted off from the
tube, the following procedure should be used. Part the
tube approximately 80-90% of the way through, remove
faceplate and tube from the lathe and knife cut the
bearing from the tube.
If the bearing is mounted in a lathe, it should be
completely machined without stopping for extended
periods of time. This prevents the bearing drooping
or going out of round under its own weight.
NOTE: Ensure that the tube is securely mounted to the faceplate
before turning. Failure to mount the tube securely could result in
the tube coming loose and causing personal injury.
44
iv) Parting to Length
Thordon can be parted to length with a standard parting
tool, however, additional rake and side clearance are
helpful to prevent heat generation resulting from the
Thordon contacting the side of the parting tool. Cuttings
from Thordon should be constantly removed during parting
off, in order to achieve a uniform cut face.
NOTE: Due to the very elastic nature of the material, caution should be
taken when removing cuttings from the work area.
MACHINING
v) Machining Lubrication Grooves
Lubrication grooves can be machined by hand or with
a router.
To machine lubrication grooves by hand, a formed tool bit
is mounted to the lathe boring bar and manually pushed
through the bearing. Several passes may be required to
achieve the final groove depth.
The outside diameter of the chuck can be divided and
marked to act as a guide for locating the grooves in
the bearing.
NOTE: Lubrication grooves must always be machined before the
bearing is fitted into the housing. Bearing I.D. can sometimes be
machined after fitting into the housing, but grooves cannot.
vi) General Machining Tips
1. To obtain optimum dimensional and surface finish
results the final machining cut should be 1.5mm
(0.060”) to 2.5mm (0.100”) and the cutting tool
razor sharp.
2. Machining must be performed in a temperature
controlled environment with minimal heat build up.
Changes in temperature can result in significant
dimensional changes.
3. Due to the elastomeric nature of Thordon, if a
machining error is made on the I.D. and if the wall
thickness if still adequate, it may be possible to
recalculate the O.D. of the bearing and still use it.
Contact Thordon Bearings for corrected O.D. value.
The grooves can be machined much more easily by
mounting a router to the boring bar and then machining
to the correct depth in one pass through the bearing.
4. Before making a final machining cut, the bearing
should be checked to ensure that it has not retained
any heat from previous cuts. If the temperature of
the bearing is higher than the machine shop ambient,
the resulting final cut dimensions will not be correct.
45
MACHINING
c) MACHINING COMPOSITE
Machining Thordon Composite is different from machining
Thordon XL, SXL or COMPAC because of the softer (black)
bearing wear surface material, GM2401. The O.D. or yellow
shell, can be machined using the same techniques as
outlined in section (b) Machining XL, SXL and COMPAC.
The I.D., however, machines differently and is covered
in this section.
i)
NOTE: It is very important to note that the final pass must be made
at the same depth, speeds and feed rate as the preceding one.
Otherwise the wear on the tool bit producing the taper will change
and the correction that is being made by hand will not be correct.
Machining the I.D. results in a burr at the lubrication
grooves that can be removed using emery cloth or a
deburring tool. The surface finish of the bearing will be
somewhat rough but the bearing will bed in quickly and
perform well.
Cutting Tool
The new Kennametal or equivalent Titanium Nitride PVD
carbide coated tool bits described earlier in the section
on machining XL, SXL or COMPAC are highly recommended
for machining Thordon Composite bearings. With these
tool bits, the black GM2401 I.D. of the bearing material
can be finish machined to an acceptable surface finish
without using a grinding hog as was recommended in
the past.
If a conventional high speed cutting tool is used for
machining the inner Composite bearing material it should
be made to the configuration illustrated below. As with
other types of Thordon, it is essential that the cutting
tool is kept sharp.
Deburring tool
ii) Machining Feeds and Speeds
Suggested turning speeds for Composite bearings
of various diameters are given in the chart below.
High Speed Steel Cutting Tool
High Speed Steel Cutting Tool
10
Bearing Diameter
Metric Imperial RPM
150mm
300mm
450mm
600mm
750mm
900mm
12.7 mm.
1/16&quot; R
1.5 mm.
3/16&quot; R
5 mm.
60˚
60˚
32˚
When using a conventional high speed tool bit to
machine the I.D. of a Thordon Composite bearing some
extra steps must be taken. Due to the nature of the
GM2401 wear surface material, conventional tool bits
wear very quickly. In the course of one machining pass
through the I.D., the tool bit will wear enough to
produce a taper along the bearing I.D. This taper must
be corrected for on a second pass, so the first step is to
ensure that two final passes in a range of 2.0 to 3.0mm
(0.080” to 0.120”) deep are required to finish machine
the I.D. of the bearing. The first pass is used to measure
the amount of taper that is occurring (a taper of 0.15mm
(0.006”) over the length of a standard Thordon tube is
common) and then this taper must be corrected for on
the second pass.
46
Feed HSS
Feed Tipped Tool
500&quot; SQ. HIGH SPEED STEEL
6”
12”
18”
24”
30”
36”
250
100
75
60
50
40
0.5mm/rev.
(0.020”/rev.)
0.25mm/rev.
(0.010”/rev.)
NOTE 1: The turning, feed and grinding speeds are provided as a guide
only. The optimum speed may vary higher or lower depending on such
variables as the length of tube, the wall thickness and how the bearing
is being supported. As is common with all machining operations, some
experimentation may be required to obtain optimum results.
NOTE 2: Cutting lubricants are not required and are not recommended.
iii) Machining Procedure (O.D. up to 250mm (10”))
The procedure for machining Thordon Composite bearings
up to 250mm (10”) O.D. can be summarized in the
following steps.
a) Part the bearing oversize and face to the required
finished length.
b) Mount the bearing on centres and rough machine
the O.D.
c) Press the bearing (light press fit) into a housing
to support it and finish machine the I.D.
MACHINING
d) Lightly press the bearing onto a mandrel and finish
machine the O.D.
iv) Machining Procedure (O.D. larger than
250 mm (10”))
Composite bearings larger than 250mm (10”) should be
machined by mounting them to a faceplate and then
machining the I.D., machining the O.D., parting oversize
and facing to length.
NOTE: Ensure that the bearing is securely mounted to the faceplate
before turning. Failure to mount the bearing securely could result in
it coming loose and causing personal injury.
d) DIMENSIONAL AND
SURFACE FINISH MEASUREMENTS
i)
Dimensional Measurements
Pi tape
shipping. The bearing may appear to be out of tolerance
due to the fact that it has gone out of round. This is
not a problem because, when the bearing is pressed into
a round housing, it will conform to the shape of the
housing and will be round. To accurately measure the
bearing outside the housing, use a pi tape to measure the
O.D. and then measure the wall thickness using a ball
micrometer to obtain the correct I.D. dimension.
A pi tape is a precision steel tape calibrated to measure
diameters by measuring circumference.
ii) Surface Finish
Outside micrometer
In most cases Thordon can be measured using the same
instruments and methods as any other material. It must
be remembered that Thordon is an elastomer and a
light touch must be used when measuring because it
is possible to deform the bearing out of round. In
addition, Thordon has a high coefficient of expansion
compared to metals, so measurements must be taken
at machine shop temperature. If this is not possible
then the dimensions must be corrected for the thermal
expansion and contraction that has occurred because
of the difference between the machine shop and
ambient measuring temperatures. Temperature charts
can be produced from the Thordon Bearing Sizing
Calculation Program.
In the case of larger diameter, relatively thin wall
bearings that have been machined and removed from the
lathe, it is quite common to find that they go oval.
This deformation can be the result of the bearing sagging
under its own weight or from being secured to a pallet for
Thordon, due to its non-metallic elastomeric nature, cannot
be machined to as smooth a surface finish as metals.
This is not a problem because the bearing goes through
a normal break in period during which the initial surface
roughness is worn smooth. It is important, however, to
strive for as smooth a surface finish as possible to reduce
friction and initial break in wear. The mechanics of
obtaining a good surface finish have been covered in
the machining section but it is important to know how
to measure the surface finish of a Thordon bearing.
Visual comparator
The quality of the Thordon surface finish should be
determined by use of a visual comparator, not by use
of a stylus device.
47
MACHINING
iii) Machining and Surface Finish Tolerances
Thordon is a non-metallic and consequently cannot
be machined to the same tight tolerances as bronze or
other rigid materials. Conversely, tight metallic tolerances
are not necessary to obtain optimum performance. The
standard Thordon machining tolerances are as follows:
Bearings up to 330mm (13.00”)
O.D. +0.13mm, -0.00mm (+0.005”, -0.000”)
I.D. +0.13mm, -0.00mm (+0.005”, -0.000”)
Bearings between 330 and 530mm (13.00” and 21.00”)
O.D. +0.18mm, -0.00mm (+0.007”, -0.000”)
Wall thickness (W.T.)
+0.00mm, -0.13mm (+0.000”, -0.005”)
I.D.(Composite only)
+0.18mm, -0.00mm (+0.007”, -0.000”)
Bearings over 530mm (21.00”)
O.D. +0.25mm, -0.00mm (+0.010”, -0.000”)
W.T. +0.00mm, -0.13mm (+0.000”, -0.005”)
I.D. (Composite only)
+0.25mm, -0.00mm (+0.010”, -0.000”)
Bearing Length Tolerance:
For bearings shorter than 500mm (20”) long
+0.00mm, -0.50mm (+0.000”, -0.020”)
For bearings longer than 500mm (20”)
+0.00mm, -1.00mm (+0.000”, -0.040”)
NOTE 1: For Thordon XL, SXL and COMPAC bearings over 330mm (13&quot;),
machined I.D. tolerance should be controlled by controlling the wall
thickness of the bearing. For Composite bearings over 330mm (13&quot;) only,
the actual I.D. of the bearing should be controlled.
NOTE 2: If the wall thickness is less than 25mm (1”) then there may be
restrictions as to the length of bearing that can be properly machined.
Consult Thordon Bearings for details.
NOTE 3: If an application requires tolerances that are tighter than those
Thordon Bearings for guidance.
The tolerances on surface finish are as follows:
XL, SXL, HPSXL, COMPAC: 3.2 micro-metres Ra
(125 micro-inches) Ra
Composite: 4.2 micro-metres Ra
(175 micro-inches) Ra
NOTE: Due to the unique characteristics of Thordon, compared to metals,
optimal performance can still be obtained at relatively high (compared
to metal) surface finishes.
48
Appendix 1
APPENDIX 1 – BONDING
WITH TG-75
Best Practices for Mixing, Preparing
and Applying
Background: Bonding of Thordon bearings into housings
is an alternative method to interference fitting. Bearings
are typically bonded when; a) the housing is out of round
or irregular, b) there are recesses in the housing that
would not provide adequate bearing support, c) when
the bearing wall is too thin for interference fit, and d) to
control tolerances and installed clearances (wall thickness
is reduced). TG-75 is a tough, high strength two part
epoxy adhesive developed to bond Thordon materials
to metal substrates.
The strength of the cured TG-75 bond is highly dependent
on several factors including, but not limited to;
a) surface preparation and cleanliness of the substrates,
b) adequate mixing of the two components,
c) curing temperature and time,
d) application procedures,
e) installation of the bearing into housing after
application.
This document outlines the procedures to ensure that
proper mixing of the TG-75 components is attained;
proper preparation of both Thordon and metal substrates
is achieved; and the correct application and installation
procedures are followed to obtain the highest bond
strength possible.
Please also refer to the BEARING TECHNOLOGY TRAINING
CD featuring the video, “Bonding Procedure” for further
instructions.
Best Practices: The following procedure should be
followed to achieve the highest level of bond integrity
possible.
Surface Preparation
The metal substrate and the Thordon material need to
be properly prepared. Poor substrate preparation may
result in loss of bond strength and the possibility of
the bearings coming loose from their housings during
operation.
Metal Preparation
Metal surfaces should be machined not smoother than
3.0 micrometers (125 micro-inches) Ra. The surface should
be gritblasted to increase adhesion. For metals exhibiting
corrosion, the surface should be clean blast to obtain
a Near White Blast clean surface per Standard SSPC-SP
No. 10/NACE No.2.
NOTE: Bonding should take place within 2 hours of surface preparation
and cleaning. For Aluminum and Stainless Steel, reduce the exposure
time to 30 minutes or less, as an oxidation layer may form very quickly
in these materials after sandblasting.
The surface to be bonded needs to be cleaned after
sandblasting with an organic solvent/degreaser such
as Methyl Ethyl Ketone (MEK), isopropyl alcohol, or
other equivalent non-residue degreaser, to remove any
contamination prior to applying the TG-75 adhesive.
Allow the degreaser to completely evaporate without
further contamination before bonding. Do not touch
the cleaned parts – if the parts need to be handled,
use NEW latex gloves to protect the clean surface from
contamination caused by oil in skin.
Thordon Surface Preparation
Thordon bearings should be machined before bonding.
The surface finish of the Thordon bearing to be bonded
should be between 3.0 to 6.0 micrometers (125 to
250 micro-inches) Ra.
It is recommended that the bearing surface be wiped
with a cloth or soft paper wetted with a small amount
of solvent – ensure that no residue from the paper is
left behind. A clean brush can also be used to clean
the surface. Allow the solvent to dry completely before
applying the adhesive. Note that the Thordon elastomeric
bearing should NOT be soaked in the solvent.
TG-75 adhesive is a two-part system consisting of an
accelerator denoted as “TG-75A” and a resin “TG-75B”.
These two components should be mixed using the
following VOLUME ratio:
Part A to Part B = 1:2
Improper mixing ratios may result in failure of the
does not harden) or it could cure too quickly (if too much
accelerator is used) resulting in significantly reduced
curing times.
Temperature of the materials at the time of mixing is
also very important for proper performance. For cartridges
stored at low temperatures, the cartridge should be
overnight) PRIOR to mixing of Parts A &amp; B. See Storage
Once mixed, the adhesive offers a maximum working time
of 60 minutes at 23&deg;C (73&deg;F) and has a viscosity of
approximately 50,000 cps. Increases in temperature will
reduce the working time or pot life.
49
Appendix 1
TG-75 adhesive is packaged in pre-measured tubes and
each tube yields 450 ml (0.12 US gallons) of mixed
adhesive. Typical coverage for one tube is 7000 cm2
(1085 in.2) at a thickness of 0.25 mm (0.010 in.).
Recommended adhesive thickness ranges from 0.25 mm
to 0.38 mm (0.010 in. to 0.015 in.). Exceeding the
recommended adhesive thickness reduces the bond
strength. Consult with Thordon Bearings if higher
adhesive thickness values must be used.
Dispensing Procedure A – Pneumatic Gun
(available from Thordon Bearings)
1. Fully retract the pistons manually: The pneumatic gun
must be connected to the airline and the middle rod
pulled back until the pistons are fully retracted.
Hold the cartridge tips over a disposable surface.
Depress the gun trigger and slowly open (turn the
regulator knob clockwise) until compound extrudes
evenly from the cartridge tips. Release the trigger.
4. Dispensing: open the pressure regulator from the lowpressure setting until the desired flow rate is obtained.
The contents of both cylinders should be fully emptied
into a disposable container and thoroughly mixed until
the colour of the adhesive is completely uniform.
Dispensing Procedure B – Manual Gun
(available from Thordon Bearings)
1. Fully depress the thumb release lever and then retract
the piston carriage assembly. See Figure 3.
2. Insert the cartridge assembly: Place the open end of the
cartridge assembly over the piston pads. Be careful to
align the pads in the centre of the cartridge plungers.
If the pistons are not centred, the plungers may flip or
be pushed unevenly resulting in improper mixing and
leaking. Snap the front end of the cartridge assembly
into position at the front of the gun. Manually push
the piston forward until they bottom out against the
inside of the cartridge plungers. See Figure 1.
Figure 3: Thumb release lever – shown with arrow.
Figure 1: TG-75 cartridge properly inserted into
pneumatic gun
3. Phase the cartridge: use a pneumatic gun with a
maximum pressure of 0.70 MPa (100 psi), turn the
regulator knob counterclockwise to the stop. Remove
the “D” shaped plugs from the cartridge - see Figure 2.
Figure 2: Plugs for TG-75 cartridge.
50
2. Insert the cartridge assembly: remove the “D” shaped
plugs from the cartridge, keep in a safe place for restorage. Place the open end of the cartridge assembly
the centre of the cartridge plungers. See Figure 4.
Figure 4: Plungers in manual gun – shown with arrows.
Appendix 1
If the pistons are not centred, the plungers may flip or
be pushed unevenly resulting in improper mixing and
leaking. Snap the front end of the cartridge assembly
into position at the front of the gun. Manually push
the piston forward until they bottom out against the
inside of the cartridge plungers.
3. Place the cartridge tips over a disposable surface and
squeeze the trigger handle slowly until compound
extrudes from both cartridge tips. Release the trigger
handle and depress the thumb release lever.
4. Maintain consistent pressure on the trigger handle
and dispense all the contents of the cylinders into a
disposable container. Thoroughly mix until the colour
of the adhesive is completely uniform.
Provided the material was mixed correctly, the cure time
for TG-75 is dependent upon the temperature during the
curing period. The recommended curing temperatures for
TG-75 are:
• Typical: 20&deg;C to 40&deg;C (68&deg;F to 104&deg;F)
• Minimum: 10&deg;C (50&deg;F)
next day. Using the thermal coefficient of expansion for
SXL [21.1x10-5 cm/cm/&deg;C (11.7x10-5 in./in./&deg;F)] and the
temperature difference 5&deg;C (9&deg;F), the bearing OD at 35&deg;C
(95&deg;F) has increased to 249.76 mm (9.833 in.). The
adhesive thickness is reduced to 0.12 mm (0.005 in.)
with the temperature difference. Such thermal effects
are even greater with larger bearings.
As mentioned previously, for best results it is
recommended to conduct the bonding installation at the
SAME temperature at which the bearing was machined.
In cold weather environments, it is important to maintain
the temperature above 10&deg;C (50&deg;F) for proper curing of
Split Bearings or Flat Surfaces
1. Apply masking or painters tape to metal edges and
ends where adhesive will not be required. Apply the
adhesive to the prepared surface of the metal and
bearing O.D. spreading evenly with a spatula or a small
notched trowel. See Figures 5 and 6.
If TG-75 is applied at temperatures outside the range
cure times.
Curing Times and Temperature
Over 60% of the bond strength is attained in 8 hours at
23&deg;C (73&deg;F). Approximately 80% of the bond strength is
achieved in 4 hours at 40&deg;C (104&deg;F). Full cure is reached
in 5 days at 23&deg;C (73&deg;F).
Insufficient curing time, particularly at low temperatures,
prior to water immersion will result in reduced bond
strength values. Water will stop further curing of
After application of adhesive, keep bearing and
carrier assembly at a constant temperature while the
Figure 5: Adhesive applied to split metal housing.
NOTE: For bearings with large outside diameter (OD) of 250 mm
(9.8 in.) and greater, it is important to machine the bearing AND
perform the bonding installation at approximately the SAME temperature.
Machining the bearing at one temperature and installing it at a different
temperature may have significant effects on the optimal adhesive
thickness – see the following example.
Example: Effect of Temperature on Adhesive Thickness
A Thordon SXL bearing is machined in the afternoon at
30&deg;C (86&deg;F) to suit a housing ID of 250 mm (9.843 in.).
Based on optimal adhesive thickness, the bearing OD
is machined to 250 mm – 2 x 0.25 mm = 249.50 mm
(9.843 in. -2 x 0.010 in. = 9.823 in).
The bearing is to be installed the next day. However, the
shop temperature has increased to 35&deg;C (95&deg;F) on the
Figure 6: TG-75 applied to OD of split SXL bearing.
51
Appendix 1
2. Position the Thordon component and clamp so that
a small amount of the adhesive is extruded out from
the edges of the Thordon part. See Figure 7. Do not
machine or handle the bonded piece for a minimum
of 8 hours at 23&deg;C (73&deg;F). Avoid smearing the
from the tape for easy tape removal once the adhesive
has cured.
Figure 8: Wire used to keep bearing concentric in housing.
Note: drawing not to scale.
Troubleshooting
1. If compound bypasses the plungers and leaks from the
backside of the cartridges, check that the plungers are
seated squarely against the cartridge plungers.
2. If the compound leaks around the retaining nut,
ensure that the nut is not cross-threaded and
tighten it further.
3. The dispensed compound must be consistent in colour.
Clean Up
Figure 7: Clamping SXL, with slight force, to metal housing.
Scrape off excess adhesive with a trowel, then clean
surface with a dry cloth to carefully remove the remainder
of the adhesive from the bonded assembly edges.
Cylindrical Bearings
Storage of TG-75 &amp; Shelf Life
1. The bearing should be sized to allow for a 0.25 mm to
0.38 mm (0.010 in. to 0.015 in.) adhesive thickness.
This is an allowance of 0.50 mm to 0.76 mm (0.020 in.
to 0.030 in.) on the outside diameter. TG-75 will fill
gaps up to a thickness of 3.0 mm (0.125 in.) but the
shear strength of the adhesive decreases at thickness
over 0.6 mm (0.025 in.).
TG-75 cartridges can be stored at room temperature,
approx. 20&deg;C (68&deg;F), with a shelf life of 15 months from
time of delivery. To increase the shelf life of the material,
the cartridges can be placed in a fridge or freezer.
The lower temperature increases the shelf life of the
unmixed components to 30 months from time of delivery.
2. Apply the adhesive to both the metal and Thordon.
Spread evenly with a spatula or small notched trowel.
3. Slide the bearing into the housing. Slight rotation of
the bearing can help homogenize the adhesive layer,
but do not use excessive back-and-forth movements
as this could induce the creation of air bubbles within
the layer.
4. Spacers can be used in situations where the bearing
cannot be held concentrically with the housing and
metal shims and wire can be used to ensure an even
thickness throughout the circumference – see Figure 8
for suggested set up.
Storage at lower temperatures, -10&deg;C to -20&deg;C (14&deg;F
to -4&deg;F) may cause the adhesive to crystallize or solidify,
giving the product the appearance of a hazy liquid or
waxy semi-solid. Crystallization is not an indication of
material problems and does not affect the performance
of the material. However, crystallization MUST be
reversed before usage, otherwise Parts A and B should
not be mixed.
This crystallization phenomenon is reversible by bringing
the materials back to room temperature. If time permits,
allow the material to warm up naturally overnight. Gentle
warming (no direct heat or flame) of the cartridge and its
contents is acceptable. Bring the cartridge to 50&deg;C
(120&deg;F) for approximately 30 minutes. Allow to cool back
to room temperature prior to use.
NOTES:
• TG-75 does not contain volatile photochemical reactive solvents.
• Produced CFC free.
• MSDS available upon request
52
WARRANTY
LIMITED WARRANTY AND LIMITATION OF LIABILITY
FOR THORDON BEARINGS INC. (‘TBI’)
(a) Basic Terms. TBI provides a limited warranty on the
Goods of its own manufacture sold by it to the Buyer
thereof, against defects of material and workmanship
(the “Limited Warranty”).
(b) Coverage. This Limited Warranty covers the repair
or replacement or the refund of the purchase price,
as TBI may elect, of any defective products regarding
which, upon discovery of the defect, the Buyer has given
immediate written notice. TBI does NOT warrant the
merchantability of its product and does NOT make any
warranty express or implied other than the warranty
contained herein.
(c) Third Party Products. Accessories, equipment and
parts not manufactured by TBI are warranted or otherwise guaranteed only to the extent and in the manner
warranted or guaranteed to TBI by the actual
manufacturer, and then only to the extent TBI is able
to enforce such warranty or guarantee.
(d) Limited Liability. TBI’s liability for any and all claims,
damages, losses and injuries arising out of or relating to
its performance or breach of any contract of sale of goods
and the manufacture, sale delivery, re-sale, repair, or use
of any goods, shall NOT exceed the agreed price of such
Goods. The Buyer’s remedy shall be at TBI’s option, the
replacement or repair of the Goods. This shall be the
Buyer’s sole, exclusive and only remedy against TBI. IN NO
EVENT SHALL TBI BE LIABLE FOR INCIDENTAL, SPECIAL OR
CONSEQUENTIAL DAMAGES, INCLUDING BUT NOT LIMITED
TO LOSS OF PROFITS, BUSINESS, GOODWILL, INCURRING
OF MACHINERY DOWNTIME, DESTRUCTION OR LOSS OF ANY
CAPITAL GOODS, LIABILITY FOR PERSONAL INJURY, DEATH,
PROPERTY DAMAGE AND ANY OTHER TYPE OF DAMAGES
WHETHER SIMILAR TO OR DIFFERENT FROM THIS LISTING.
(e) Latent Defects. In cases of defects in materials or
workmanship or defects arising from the selection of
material or processes of manufacturer, such defects must
be apparent in the Goods within three (3) months, after
delivery and acceptance of the Goods to the Buyer.
(f) Exclusions. TBI shall, as to each aforesaid defect, be
relieved of all obligations and liability under this Limited
Warranty if:
2. The Goods shall not be operated or maintained in
accordance with TBI’s written instructions as delivered
to the Buyer, at any time or from time to time,
unless the Buyer furnishes reasonable evidence
that such operation or maintenance was not a cause
of the defect;
3. The Goods shall not be operated or maintained
under normal industry use, unless the Buyer furnishes
reasonable evidence that such operation was not a
cause of the defect;
4. The Goods shall have been repaired, altered or
modified without TBI’s written approval or, if the
Goods shall have been operated subsequent to its
involvement in an accident or breakdown, unless the
Buyer furnishes reasonable evidence that such repair,
alteration, modification, operation, accident or
breakdown was not a cause of the defect; provided,
however, that this limitation insofar as it relates
to repairs, accidents and breakdowns, shall NOT be
applicable to routine repairs or replacements or minor
accidents or minor breakdowns which normally occur
in the operation of a machine, if such repairs or
replacements are made with suitable materials and
according to standard practice and engineering;
5. The Buyer does not submit reasonable proof to TBI
that the defect is due to a material embraced within
TBI’s Limited Warranty hereunder.
(g) Warranty Term. This Limited Warranty made by TBI
contained in these Terms and Conditions, or contained in
any document given in order to carry out the transactions
contemplated hereby, shall continue in full force and
effect for the benefit of the Buyer, save and except, no
the date which is twelve (12) months following delivery
and acceptance of the Goods pursuant to this Contract.
(h) Expiration and Release. After the expiration of this
Limited Warranty’s period of time, as aforesaid, TBI shall
be released from all obligations and liabilities in respect
of such warranty made by TBI and contained in this
Contract or in any document given in order to carry out
the transactions contemplated hereby.
1. The Goods are operated with any accessory,
equipment or part not specifically approved by TBI
and not manufactured by TBI or to TBI’s design and
specifications, unless the Buyer furnishes reasonable
evidence that such installation was not a cause of
the defect; provided, that this provision shall not
apply to any accessory, equipment or part, the use
of which does not effect the safety of the Goods;
53
Customer Focused To Support
Supply and Service: Geared to provide quick
response to customer needs, Thordon
Bearings understands the importance of fast
delivery and reduced down time. Thordon
marine and industrial bearings can be
designed, produced to the exact requirements
of the customer and shipped quickly.
Manufacturing: Thordon’s modern
polymer processing facility is staffed with
experienced and dedicated employees.
Bearings up to 2.2 m (86&quot;) in diameter have
been supplied and bearings up to 1.5 m
(60&quot;) O.D. can be machined in-house.
Distribution: With Thordon bearings
specified all around the world, an extensive
distribution network has been established in
over 70 countries. Inventories of common
bearing sizes are stocked by local Thordon
Distributors and are backed up by large
regional and head office Thordon stocks.
Quality: Thordon Bearings Inc. is a
9001:2000 Quality System requirements.
With over 35 years experience in
elastomeric bearing design, application
engineering and manufacturing, Thordon
marine and industrial bearings are
recognized worldwide for both quality
and performance.
Research and Development: Thordon
bearings are being continuously tested by our
Bearing Test Facility. The Facility evaluates
new designs and applications before they are
put into service. Ongoing testing not only
allows for design refinements, but ensures
quality and performance after installation.
Our polymer laboratory evaluates new and
modified polymers in a continuing quest to
improve Thordon bearing performance and
searches for new polymer bearing solutions.
Application
Engineering:
Thordon
Bearing’s engineers work closely with
customers to provide innovative bearing
system designs that meet or exceed the
technical requirements of the application.